# Supplementary Material for CrystEngComm
# This journal is (c) The Royal Society of Chemistry 2009

data_global
_journal_name_full               CrystEngComm

_journal_coden_Cambridge         1350

_publ_contact_author_name        'Zhong-Min Su'
_publ_contact_author_email       ZMSU@NENU.EDU.CN

_publ_section_title              
;
Construction and property investigation of
transition-metal-complexes modified octamolybdate hybrid materials
based on V-shaped organic ligands
;
loop_
_publ_author_name
'Zhong-Min Su'
'Ya-Qian Lan'
'Kui-Zhan Shao'
'Xin-Long Wang'
;
Guang-Juan Xu
;
'Guang-Sheng Yang'
'Hong-Ying Zang'

# Attachment '1-5.cif'

data_1
_database_code_depnum_ccdc_archive 'CCDC 727450'

_audit_creation_method           SHELXL-97
_chemical_name_systematic        
;
?
;
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         'C18 H24 Cu Mo8 N6 O28'
_chemical_formula_sum            'C18 H24 Cu Mo8 N6 O28'
_chemical_formula_weight         1603.49

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cu Cu 0.3201 1.2651 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_symmetry_cell_setting           Triclinic
_symmetry_space_group_name_H-M   P-1

loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, -z'

_cell_length_a                   9.7380(9)
_cell_length_b                   10.415(1)
_cell_length_c                   10.660(1)
_cell_angle_alpha                107.409(1)
_cell_angle_beta                 90.801(1)
_cell_angle_gamma                115.658(1)
_cell_volume                     916.86(15)
_cell_formula_units_Z            1
_cell_measurement_temperature    293(2)
_cell_measurement_reflns_used    'total reflection'
_cell_measurement_theta_min      1.33
_cell_measurement_theta_max      26.04

_exptl_crystal_description       block
_exptl_crystal_colour            black
_exptl_crystal_size_max          0.48
_exptl_crystal_size_mid          0.36
_exptl_crystal_size_min          0.28
_exptl_crystal_density_meas      ?
_exptl_crystal_density_diffrn    2.897
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             759
_exptl_absorpt_coefficient_mu    3.319
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_correction_T_min  0.246
_exptl_absorpt_correction_T_max  0.396
_exptl_absorpt_process_details   'SADABS (Sheldrick, 1996)'

_exptl_special_details           
;
?
;

_diffrn_ambient_temperature      293(2)
_diffrn_radiation_wavelength     0.71069
_diffrn_radiation_type           MoK\a
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_monochromator  graphite
_diffrn_measurement_device_type  'Bruker SMART APEX II CCD area-detector'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_detector_area_resol_mean ?
_diffrn_standards_number         0
_diffrn_standards_interval_count ?
_diffrn_standards_interval_time  0
_diffrn_standards_decay_%        ?
_diffrn_reflns_number            4635
_diffrn_reflns_av_R_equivalents  0.0109
_diffrn_reflns_av_sigmaI/netI    0.0226
_diffrn_reflns_limit_h_min       -11
_diffrn_reflns_limit_h_max       7
_diffrn_reflns_limit_k_min       -11
_diffrn_reflns_limit_k_max       12
_diffrn_reflns_limit_l_min       -12
_diffrn_reflns_limit_l_max       12
_diffrn_reflns_theta_min         2.03
_diffrn_reflns_theta_max         25.00
_reflns_number_total             3186
_reflns_number_gt                2727
_reflns_threshold_expression     >2sigma(I)

_computing_data_collection       'Bruker SMART'
_computing_cell_refinement       'Bruker SMART'
_computing_data_reduction        'Bruker SMART'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'

_refine_special_details          
;
Refinement of F² against ALL reflections. The weighted R-factor wR and
goodness of fit S are based on F², conventional R-factors R are based
on F, with F set to zero for negative F². The threshold expression of
F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is
not relevant to the choice of reflections for refinement. R-factors based
on F² are statistically about twice as large as those based on F, and R-
factors based on ALL data will be even larger.
;

_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'calc w=1/[σ²(Fo²)+(0.0575P)²+7.5576P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_atom_sites_solution_hydrogens   geom
_refine_ls_hydrogen_treatment    constr
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       ?
_refine_ls_number_reflns         3186
_refine_ls_number_parameters     267
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0465
_refine_ls_R_factor_gt           0.0402
_refine_ls_wR_factor_ref         0.1139
_refine_ls_wR_factor_gt          0.1092
_refine_ls_goodness_of_fit_ref   1.060
_refine_ls_restrained_S_all      1.060
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Cu1 Cu 0.5000 1.0000 1.0000 0.0409(4) Uani 1 2 d S . .
Mo1 Mo 0.30051(7) 0.71564(7) 0.64237(6) 0.02313(18) Uani 1 1 d . . .
Mo2 Mo 0.08254(6) 0.37095(7) 0.46249(6) 0.02089(17) Uani 1 1 d . . .
Mo3 Mo -0.23292(7) 0.16603(7) 0.59007(6) 0.02654(18) Uani 1 1 d . . .
Mo4 Mo 0.01524(7) 0.48180(7) 0.22610(6) 0.02317(18) Uani 1 1 d . . .
C1 C 0.7348(12) 0.9412(11) 1.0980(10) 0.055(3) Uani 1 1 d . . .
H1 H 0.7141 0.9693 1.1842 0.066 Uiso 1 1 calc R . .
C2 C 0.7318(10) 0.9003(10) 0.8827(9) 0.042(2) Uani 1 1 d . . .
H2 H 0.7067 0.9006 0.7983 0.051 Uiso 1 1 calc R . .
C3 C 0.8267(10) 0.8453(9) 0.9114(9) 0.044(2) Uani 1 1 d . . .
H3 H 0.8759 0.7994 0.8538 0.052 Uiso 1 1 calc R . .
C4 C 0.9018(16) 0.8342(16) 1.1439(14) 0.085(4) Uiso 1 1 d . . .
H5 H 0.9725 0.9237 1.2166 0.102 Uiso 1 1 calc R . .
H4 H 0.9595 0.7842 1.0973 0.102 Uiso 1 1 calc R . .
C5 C 0.7703(14) 0.7246(13) 1.1996(12) 0.061(3) Uani 1 1 d . . .
C6 C 0.6793(11) 0.5757(10) 1.1252(10) 0.050(2) Uani 1 1 d . . .
H6 H 0.7011 0.5356 1.0421 0.060 Uiso 1 1 calc R . .
C7 C 0.5559(12) 0.4839(12) 1.1712(12) 0.059(3) Uani 1 1 d . . .
H7 H 0.4932 0.3825 1.1218 0.070 Uiso 1 1 calc R . .
C8 C 0.5314(11) 0.5513(13) 1.2943(11) 0.052(3) Uani 1 1 d . . .
H8 H 0.4489 0.4990 1.3321 0.062 Uiso 1 1 calc R . .
C9 C 0.7393(16) 0.764(2) 1.3054(16) 0.087(5) Uani 1 1 d . . .
H10 H 0.8056 0.8626 1.3596 0.105 Uiso 1 1 calc R . .
O1 O -0.1187(7) 0.3954(6) 0.0853(5) 0.0374(13) Uani 1 1 d . . .
O2 O 0.1758(6) 0.4724(6) 0.1750(5) 0.0343(12) Uani 1 1 d . . .
O3 O 0.0723(6) 0.6889(5) 0.2613(5) 0.0255(10) Uani 1 1 d . . .
O4 O -0.0555(5) 0.3127(5) 0.3004(5) 0.0245(10) Uani 1 1 d . . .
O5 O 0.1244(5) 0.5901(5) 0.4519(5) 0.0232(10) Uani 1 1 d . . .
O6 O -0.0129(6) 0.2037(6) 0.4984(5) 0.0294(11) Uani 1 1 d . . .
O7 O -0.3838(6) 0.1858(7) 0.6555(6) 0.0385(13) Uani 1 1 d . . .
O8 O -0.2510(7) -0.0016(6) 0.5970(6) 0.0435(14) Uani 1 1 d . . .
O9 O 0.2386(6) 0.3624(6) 0.4007(5) 0.0333(12) Uani 1 1 d . . .
O10 O 0.1763(5) 0.5071(5) 0.6442(5) 0.0238(10) Uani 1 1 d . . .
O11 O 0.4457(6) 0.6907(6) 0.5707(5) 0.0321(12) Uani 1 1 d . . .
O12 O 0.3012(6) 0.8762(6) 0.5944(5) 0.0301(11) Uani 1 1 d . . .
O13 O 0.3770(6) 0.8103(6) 0.8084(5) 0.0334(12) Uani 1 1 d . . .
N2 N 0.8333(9) 0.8756(9) 1.0556(11) 0.071(3) Uani 1 1 d . . .
N1 N 0.6287(11) 0.6912(12) 1.3551(8) 0.059(2) Uani 1 1 d . . .
H9 H 0.6172 0.7363 1.4331 0.070 Uiso 1 1 calc R . .
N3 N 0.6775(8) 0.9554(9) 0.9931(7) 0.0438(18) Uani 1 1 d . . .
O1W O 0.3910(8) 0.8307(8) 1.0868(7) 0.0549(17) Uiso 1 1 d . . .


_geom_special_details            
;
All esds (except the esd in the dihedral angle between two l.s. planes)
are estimated using the full covariance matrix. The cell esds are taken
into account individually in the estimation of esds in distances, angles
and torsion angles; correlations between esds in cell parameters are only
used when they are defined by crystal symmetry. An approximate (isotropic)
treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Cu1 N3 1.971(7) . ?
Cu1 N3 1.971(7) 2_677 ?
Cu1 O1W 2.115(7) . ?
Cu1 O1W 2.115(7) 2_677 ?
Cu1 O13 2.231(5) . ?
Cu1 O13 2.231(5) 2_677 ?
Mo1 O11 1.697(5) . ?
Mo1 O13 1.716(5) . ?
Mo1 O12 1.887(5) . ?
Mo1 O10 1.982(5) . ?
Mo1 O5 2.269(5) . ?
Mo1 O4 2.385(5) 2_566 ?
Mo1 Mo2 3.1997(8) . ?
Mo2 O9 1.692(5) . ?
Mo2 O6 1.747(5) . ?
Mo2 O4 1.940(5) . ?
Mo2 O10 1.945(5) . ?
Mo2 O5 2.177(5) . ?
Mo2 O5 2.366(5) 2_566 ?
Mo3 O7 1.700(5) . ?
Mo3 O8 1.702(6) . ?
Mo3 O12 1.922(5) 2_566 ?
Mo3 O3 1.922(5) 2_566 ?
Mo3 O6 2.293(5) . ?
Mo3 O5 2.477(5) 2_566 ?
Mo4 O2 1.696(5) . ?
Mo4 O1 1.698(5) . ?
Mo4 O3 1.891(5) . ?
Mo4 O4 2.001(5) . ?
Mo4 O5 2.337(5) . ?
Mo4 O10 2.360(5) 2_566 ?
C1 N3 1.318(12) . ?
C1 N2 1.409(13) . ?
C1 H1 0.9300 . ?
C2 C3 1.354(13) . ?
C2 N3 1.368(11) . ?
C2 H2 0.9300 . ?
C3 N2 1.468(13) . ?
C3 H3 0.9300 . ?
C4 N2 1.411(15) . ?
C4 C5 1.568(18) . ?
C4 H5 0.9700 . ?
C4 H4 0.9700 . ?
C5 C9 1.171(17) . ?
C5 C6 1.369(14) . ?
C6 C7 1.379(14) . ?
C6 H6 0.9300 . ?
C7 C8 1.369(15) . ?
C7 H7 0.9300 . ?
C8 N1 1.289(14) . ?
C8 H8 0.9300 . ?
C9 N1 1.251(15) . ?
C9 H10 0.9300 . ?
O3 Mo3 1.922(5) 2_566 ?
O4 Mo1 2.385(5) 2_566 ?
O5 Mo2 2.366(5) 2_566 ?
O5 Mo3 2.477(5) 2_566 ?
O10 Mo4 2.360(5) 2_566 ?
O12 Mo3 1.922(5) 2_566 ?
N1 H9 0.8600 . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
N3 Cu1 N3 180.000(4) . 2_677 ?
N3 Cu1 O1W 88.8(3) . . ?
N3 Cu1 O1W 91.2(3) 2_677 . ?
N3 Cu1 O1W 91.2(3) . 2_677 ?
N3 Cu1 O1W 88.8(3) 2_677 2_677 ?
O1W Cu1 O1W 180.000(2) . 2_677 ?
N3 Cu1 O13 90.6(2) . . ?
N3 Cu1 O13 89.4(3) 2_677 . ?
O1W Cu1 O13 83.9(2) . . ?
O1W Cu1 O13 96.1(2) 2_677 . ?
N3 Cu1 O13 89.4(3) . 2_677 ?
N3 Cu1 O13 90.6(3) 2_677 2_677 ?
O1W Cu1 O13 96.1(2) . 2_677 ?
O1W Cu1 O13 83.9(2) 2_677 2_677 ?
O13 Cu1 O13 180.000(2) . 2_677 ?
O11 Mo1 O13 104.7(3) . . ?
O11 Mo1 O12 102.7(2) . . ?
O13 Mo1 O12 99.3(2) . . ?
O11 Mo1 O10 98.1(2) . . ?
O13 Mo1 O10 100.4(2) . . ?
O12 Mo1 O10 146.5(2) . . ?
O11 Mo1 O5 95.4(2) . . ?
O13 Mo1 O5 159.8(2) . . ?
O12 Mo1 O5 78.00(19) . . ?
O10 Mo1 O5 74.12(18) . . ?
O11 Mo1 O4 164.9(2) . 2_566 ?
O13 Mo1 O4 87.8(2) . 2_566 ?
O12 Mo1 O4 83.1(2) . 2_566 ?
O10 Mo1 O4 70.88(17) . 2_566 ?
O5 Mo1 O4 71.97(17) . 2_566 ?
O11 Mo1 Mo2 85.77(18) . . ?
O13 Mo1 Mo2 135.43(19) . . ?
O12 Mo1 Mo2 120.83(15) . . ?
O10 Mo1 Mo2 35.05(14) . . ?
O5 Mo1 Mo2 42.84(12) . . ?
O4 Mo1 Mo2 79.33(11) 2_566 . ?
O9 Mo2 O6 104.7(3) . . ?
O9 Mo2 O4 101.3(2) . . ?
O6 Mo2 O4 97.8(2) . . ?
O9 Mo2 O10 100.8(2) . . ?
O6 Mo2 O10 97.6(2) . . ?
O4 Mo2 O10 148.8(2) . . ?
O9 Mo2 O5 98.5(2) . . ?
O6 Mo2 O5 156.8(2) . . ?
O4 Mo2 O5 78.17(19) . . ?
O10 Mo2 O5 76.99(19) . . ?
O9 Mo2 O5 173.8(2) . 2_566 ?
O6 Mo2 O5 81.5(2) . 2_566 ?
O4 Mo2 O5 78.23(18) . 2_566 ?
O10 Mo2 O5 77.43(17) . 2_566 ?
O5 Mo2 O5 75.35(19) . 2_566 ?
O9 Mo2 Mo1 88.93(19) . . ?
O6 Mo2 Mo1 133.46(17) . . ?
O4 Mo2 Mo1 123.29(14) . . ?
O10 Mo2 Mo1 35.83(14) . . ?
O5 Mo2 Mo1 45.12(12) . . ?
O5 Mo2 Mo1 86.19(11) 2_566 . ?
O7 Mo3 O8 105.7(3) . . ?
O7 Mo3 O12 99.3(3) . 2_566 ?
O8 Mo3 O12 104.4(3) . 2_566 ?
O7 Mo3 O3 98.0(2) . 2_566 ?
O8 Mo3 O3 102.4(3) . 2_566 ?
O12 Mo3 O3 142.6(2) 2_566 2_566 ?
O7 Mo3 O6 164.2(2) . . ?
O8 Mo3 O6 90.1(2) . . ?
O12 Mo3 O6 76.9(2) 2_566 . ?
O3 Mo3 O6 77.44(19) 2_566 . ?
O7 Mo3 O5 94.7(2) . 2_566 ?
O8 Mo3 O5 159.7(2) . 2_566 ?
O12 Mo3 O5 72.26(19) 2_566 2_566 ?
O3 Mo3 O5 73.46(18) 2_566 2_566 ?
O6 Mo3 O5 69.56(17) . 2_566 ?
O2 Mo4 O1 105.1(3) . . ?
O2 Mo4 O3 101.2(2) . . ?
O1 Mo4 O3 102.7(2) . . ?
O2 Mo4 O4 97.8(2) . . ?
O1 Mo4 O4 99.2(2) . . ?
O3 Mo4 O4 145.9(2) . . ?
O2 Mo4 O5 93.9(2) . . ?
O1 Mo4 O5 160.5(2) . . ?
O3 Mo4 O5 77.48(19) . . ?
O4 Mo4 O5 73.26(18) . . ?
O2 Mo4 O10 162.8(2) . 2_566 ?
O1 Mo4 O10 90.0(2) . 2_566 ?
O3 Mo4 O10 83.05(19) . 2_566 ?
O4 Mo4 O10 71.16(18) . 2_566 ?
O5 Mo4 O10 70.67(16) . 2_566 ?
N3 C1 N2 107.4(9) . . ?
N3 C1 H1 126.3 . . ?
N2 C1 H1 126.3 . . ?
C3 C2 N3 111.6(8) . . ?
C3 C2 H2 124.2 . . ?
N3 C2 H2 124.2 . . ?
C2 C3 N2 103.2(8) . . ?
C2 C3 H3 128.4 . . ?
N2 C3 H3 128.4 . . ?
N2 C4 C5 108.4(10) . . ?
N2 C4 H5 110.0 . . ?
C5 C4 H5 110.0 . . ?
N2 C4 H4 110.0 . . ?
C5 C4 H4 110.0 . . ?
H5 C4 H4 108.4 . . ?
C9 C5 C6 115.0(15) . . ?
C9 C5 C4 123.0(13) . . ?
C6 C5 C4 121.9(11) . . ?
C5 C6 C7 121.2(11) . . ?
C5 C6 H6 119.4 . . ?
C7 C6 H6 119.4 . . ?
C8 C7 C6 115.8(10) . . ?
C8 C7 H7 122.1 . . ?
C6 C7 H7 122.1 . . ?
N1 C8 C7 116.5(9) . . ?
N1 C8 H8 121.8 . . ?
C7 C8 H8 121.8 . . ?
C5 C9 N1 128.6(19) . . ?
C5 C9 H10 115.7 . . ?
N1 C9 H10 115.7 . . ?
Mo4 O3 Mo3 117.6(2) . 2_566 ?
Mo2 O4 Mo4 110.3(2) . . ?
Mo2 O4 Mo1 108.2(2) . 2_566 ?
Mo4 O4 Mo1 104.1(2) . 2_566 ?
Mo2 O5 Mo1 92.04(17) . . ?
Mo2 O5 Mo4 91.49(17) . . ?
Mo1 O5 Mo4 161.6(2) . . ?
Mo2 O5 Mo2 104.65(19) . 2_566 ?
Mo1 O5 Mo2 98.57(17) . 2_566 ?
Mo4 O5 Mo2 97.95(17) . 2_566 ?
Mo2 O5 Mo3 163.9(2) . 2_566 ?
Mo1 O5 Mo3 86.39(15) . 2_566 ?
Mo4 O5 Mo3 85.25(15) . 2_566 ?
Mo2 O5 Mo3 91.39(16) 2_566 2_566 ?
Mo2 O6 Mo3 117.6(2) . . ?
Mo2 O10 Mo1 109.1(2) . . ?
Mo2 O10 Mo4 110.6(2) . 2_566 ?
Mo1 O10 Mo4 105.6(2) . 2_566 ?
Mo1 O12 Mo3 117.2(3) . 2_566 ?
Mo1 O13 Cu1 160.4(3) . . ?
C4 N2 C1 120.6(11) . . ?
C4 N2 C3 131.3(10) . . ?
C1 N2 C3 107.6(8) . . ?
C9 N1 C8 122.8(12) . . ?
C9 N1 H9 118.6 . . ?
C8 N1 H9 118.6 . . ?
C1 N3 C2 110.2(7) . . ?
C1 N3 Cu1 120.0(6) . . ?
C2 N3 Cu1 127.9(6) . . ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
O11 Mo1 Mo2 O9 0.5(2) . . . . ?
O13 Mo1 Mo2 O9 -106.3(3) . . . . ?
O12 Mo1 Mo2 O9 102.8(3) . . . . ?
O10 Mo1 Mo2 O9 -110.2(3) . . . . ?
O5 Mo1 Mo2 O9 103.1(3) . . . . ?
O4 Mo1 Mo2 O9 178.0(2) 2_566 . . . ?
O11 Mo1 Mo2 O6 109.9(3) . . . . ?
O13 Mo1 Mo2 O6 3.1(4) . . . . ?
O12 Mo1 Mo2 O6 -147.8(3) . . . . ?
O10 Mo1 Mo2 O6 -0.8(3) . . . . ?
O5 Mo1 Mo2 O6 -147.5(3) . . . . ?
O4 Mo1 Mo2 O6 -72.6(3) 2_566 . . . ?
O11 Mo1 Mo2 O4 -102.4(2) . . . . ?
O13 Mo1 Mo2 O4 150.9(3) . . . . ?
O12 Mo1 Mo2 O4 -0.1(2) . . . . ?
O10 Mo1 Mo2 O4 147.0(3) . . . . ?
O5 Mo1 Mo2 O4 0.2(2) . . . . ?
O4 Mo1 Mo2 O4 75.1(2) 2_566 . . . ?
O11 Mo1 Mo2 O10 110.7(3) . . . . ?
O13 Mo1 Mo2 O10 3.9(3) . . . . ?
O12 Mo1 Mo2 O10 -147.1(3) . . . . ?
O5 Mo1 Mo2 O10 -146.8(3) . . . . ?
O4 Mo1 Mo2 O10 -71.8(3) 2_566 . . . ?
O11 Mo1 Mo2 O5 -102.6(3) . . . . ?
O13 Mo1 Mo2 O5 150.7(3) . . . . ?
O12 Mo1 Mo2 O5 -0.3(2) . . . . ?
O10 Mo1 Mo2 O5 146.8(3) . . . . ?
O4 Mo1 Mo2 O5 74.9(2) 2_566 . . . ?
O11 Mo1 Mo2 O5 -175.6(2) . . . 2_566 ?
O13 Mo1 Mo2 O5 77.6(3) . . . 2_566 ?
O12 Mo1 Mo2 O5 -73.4(2) . . . 2_566 ?
O10 Mo1 Mo2 O5 73.7(3) . . . 2_566 ?
O5 Mo1 Mo2 O5 -73.1(2) . . . 2_566 ?
O4 Mo1 Mo2 O5 1.88(16) 2_566 . . 2_566 ?
N3 C2 C3 N2 -2.0(10) . . . . ?
N2 C4 C5 C9 -100.8(14) . . . . ?
N2 C4 C5 C6 76.8(14) . . . . ?
C9 C5 C6 C7 3.3(15) . . . . ?
C4 C5 C6 C7 -174.4(10) . . . . ?
C5 C6 C7 C8 0.1(14) . . . . ?
C6 C7 C8 N1 -2.1(13) . . . . ?
C6 C5 C9 N1 -5.1(19) . . . . ?
C4 C5 C9 N1 172.6(12) . . . . ?
O2 Mo4 O3 Mo3 -68.4(3) . . . 2_566 ?
O1 Mo4 O3 Mo3 -176.8(3) . . . 2_566 ?
O4 Mo4 O3 Mo3 54.4(5) . . . 2_566 ?
O5 Mo4 O3 Mo3 23.1(2) . . . 2_566 ?
O10 Mo4 O3 Mo3 94.8(3) 2_566 . . 2_566 ?
O9 Mo2 O4 Mo4 -74.0(3) . . . . ?
O6 Mo2 O4 Mo4 179.3(2) . . . . ?
O10 Mo2 O4 Mo4 60.3(5) . . . . ?
O5 Mo2 O4 Mo4 22.4(2) . . . . ?
O5 Mo2 O4 Mo4 99.7(2) 2_566 . . . ?
Mo1 Mo2 O4 Mo4 22.3(3) . . . . ?
O9 Mo2 O4 Mo1 172.8(2) . . . 2_566 ?
O6 Mo2 O4 Mo1 66.0(2) . . . 2_566 ?
O10 Mo2 O4 Mo1 -53.0(4) . . . 2_566 ?
O5 Mo2 O4 Mo1 -90.8(2) . . . 2_566 ?
O5 Mo2 O4 Mo1 -13.58(18) 2_566 . . 2_566 ?
Mo1 Mo2 O4 Mo1 -90.99(19) . . . 2_566 ?
O2 Mo4 O4 Mo2 70.4(3) . . . . ?
O1 Mo4 O4 Mo2 177.2(3) . . . . ?
O3 Mo4 O4 Mo2 -53.2(4) . . . . ?
O5 Mo4 O4 Mo2 -21.3(2) . . . . ?
O10 Mo4 O4 Mo2 -96.1(2) 2_566 . . . ?
O2 Mo4 O4 Mo1 -173.7(2) . . . 2_566 ?
O1 Mo4 O4 Mo1 -67.0(3) . . . 2_566 ?
O3 Mo4 O4 Mo1 62.7(4) . . . 2_566 ?
O5 Mo4 O4 Mo1 94.58(19) . . . 2_566 ?
O10 Mo4 O4 Mo1 19.80(16) 2_566 . . 2_566 ?
O9 Mo2 O5 Mo1 -79.9(2) . . . . ?
O6 Mo2 O5 Mo1 98.1(5) . . . . ?
O4 Mo2 O5 Mo1 -179.8(2) . . . . ?
O10 Mo2 O5 Mo1 19.22(17) . . . . ?
O5 Mo2 O5 Mo1 99.4(2) 2_566 . . . ?
O9 Mo2 O5 Mo4 82.0(2) . . . . ?
O6 Mo2 O5 Mo4 -99.9(5) . . . . ?
O4 Mo2 O5 Mo4 -17.85(17) . . . . ?
O10 Mo2 O5 Mo4 -178.80(19) . . . . ?
O5 Mo2 O5 Mo4 -98.6(2) 2_566 . . . ?
Mo1 Mo2 O5 Mo4 162.0(2) . . . . ?
O9 Mo2 O5 Mo2 -179.3(2) . . . 2_566 ?
O6 Mo2 O5 Mo2 -1.3(6) . . . 2_566 ?
O4 Mo2 O5 Mo2 80.8(2) . . . 2_566 ?
O10 Mo2 O5 Mo2 -80.2(2) . . . 2_566 ?
O5 Mo2 O5 Mo2 0.0 2_566 . . 2_566 ?
Mo1 Mo2 O5 Mo2 -99.4(2) . . . 2_566 ?
O9 Mo2 O5 Mo3 4.1(8) . . . 2_566 ?
O6 Mo2 O5 Mo3 -177.9(7) . . . 2_566 ?
O4 Mo2 O5 Mo3 -95.8(8) . . . 2_566 ?
O10 Mo2 O5 Mo3 103.3(8) . . . 2_566 ?
O5 Mo2 O5 Mo3 -176.5(9) 2_566 . . 2_566 ?
Mo1 Mo2 O5 Mo3 84.1(8) . . . 2_566 ?
O11 Mo1 O5 Mo2 77.9(2) . . . . ?
O13 Mo1 O5 Mo2 -95.9(6) . . . . ?
O12 Mo1 O5 Mo2 179.7(2) . . . . ?
O10 Mo1 O5 Mo2 -19.10(17) . . . . ?
O4 Mo1 O5 Mo2 -93.70(18) 2_566 . . . ?
O11 Mo1 O5 Mo4 -23.1(8) . . . . ?
O13 Mo1 O5 Mo4 163.1(7) . . . . ?
O12 Mo1 O5 Mo4 78.8(7) . . . . ?
O10 Mo1 O5 Mo4 -120.0(8) . . . . ?
O4 Mo1 O5 Mo4 165.3(8) 2_566 . . . ?
Mo2 Mo1 O5 Mo4 -101.0(8) . . . . ?
O11 Mo1 O5 Mo2 -177.0(2) . . . 2_566 ?
O13 Mo1 O5 Mo2 9.2(7) . . . 2_566 ?
O12 Mo1 O5 Mo2 -75.1(2) . . . 2_566 ?
O10 Mo1 O5 Mo2 86.05(19) . . . 2_566 ?
O4 Mo1 O5 Mo2 11.45(16) 2_566 . . 2_566 ?
Mo2 Mo1 O5 Mo2 105.1(2) . . . 2_566 ?
O11 Mo1 O5 Mo3 -86.1(2) . . . 2_566 ?
O13 Mo1 O5 Mo3 100.1(6) . . . 2_566 ?
O12 Mo1 O5 Mo3 15.74(18) . . . 2_566 ?
O10 Mo1 O5 Mo3 176.92(19) . . . 2_566 ?
O4 Mo1 O5 Mo3 102.32(17) 2_566 . . 2_566 ?
Mo2 Mo1 O5 Mo3 -164.0(2) . . . 2_566 ?
O2 Mo4 O5 Mo2 -79.3(2) . . . . ?
O1 Mo4 O5 Mo2 87.4(7) . . . . ?
O3 Mo4 O5 Mo2 -180.0(2) . . . . ?
O4 Mo4 O5 Mo2 17.68(17) . . . . ?
O10 Mo4 O5 Mo2 93.10(18) 2_566 . . . ?
O2 Mo4 O5 Mo1 21.7(8) . . . . ?
O1 Mo4 O5 Mo1 -171.6(7) . . . . ?
O3 Mo4 O5 Mo1 -78.9(7) . . . . ?
O4 Mo4 O5 Mo1 118.7(8) . . . . ?
O10 Mo4 O5 Mo1 -165.9(8) 2_566 . . . ?
O2 Mo4 O5 Mo2 175.7(2) . . . 2_566 ?
O1 Mo4 O5 Mo2 -17.7(8) . . . 2_566 ?
O3 Mo4 O5 Mo2 75.0(2) . . . 2_566 ?
O4 Mo4 O5 Mo2 -87.33(19) . . . 2_566 ?
O10 Mo4 O5 Mo2 -11.92(15) 2_566 . . 2_566 ?
O2 Mo4 O5 Mo3 84.9(2) . . . 2_566 ?
O1 Mo4 O5 Mo3 -108.4(7) . . . 2_566 ?
O3 Mo4 O5 Mo3 -15.72(17) . . . 2_566 ?
O4 Mo4 O5 Mo3 -178.08(19) . . . 2_566 ?
O10 Mo4 O5 Mo3 -102.66(17) 2_566 . . 2_566 ?
O9 Mo2 O6 Mo3 178.7(3) . . . . ?
O4 Mo2 O6 Mo3 -77.3(3) . . . . ?
O10 Mo2 O6 Mo3 75.5(3) . . . . ?
O5 Mo2 O6 Mo3 0.8(7) . . . . ?
O5 Mo2 O6 Mo3 -0.5(2) 2_566 . . . ?
Mo1 Mo2 O6 Mo3 75.9(3) . . . . ?
O7 Mo3 O6 Mo2 -1.5(10) . . . . ?
O8 Mo3 O6 Mo2 -179.0(3) . . . . ?
O12 Mo3 O6 Mo2 76.2(3) 2_566 . . . ?
O3 Mo3 O6 Mo2 -76.3(3) 2_566 . . . ?
O5 Mo3 O6 Mo2 0.5(2) 2_566 . . . ?
O9 Mo2 O10 Mo1 72.8(3) . . . . ?
O6 Mo2 O10 Mo1 179.4(2) . . . . ?
O4 Mo2 O10 Mo1 -61.6(4) . . . . ?
O5 Mo2 O10 Mo1 -23.5(2) . . . . ?
O5 Mo2 O10 Mo1 -101.1(2) 2_566 . . . ?
O9 Mo2 O10 Mo4 -171.4(2) . . . 2_566 ?
O6 Mo2 O10 Mo4 -64.8(3) . . . 2_566 ?
O4 Mo2 O10 Mo4 54.2(5) . . . 2_566 ?
O5 Mo2 O10 Mo4 92.3(2) . . . 2_566 ?
O5 Mo2 O10 Mo4 14.71(19) 2_566 . . 2_566 ?
Mo1 Mo2 O10 Mo4 115.8(3) . . . 2_566 ?
O11 Mo1 O10 Mo2 -70.5(3) . . . . ?
O13 Mo1 O10 Mo2 -177.2(2) . . . . ?
O12 Mo1 O10 Mo2 57.6(4) . . . . ?
O5 Mo1 O10 Mo2 22.8(2) . . . . ?
O4 Mo1 O10 Mo2 98.8(2) 2_566 . . . ?
O11 Mo1 O10 Mo4 170.5(2) . . . 2_566 ?
O13 Mo1 O10 Mo4 63.8(3) . . . 2_566 ?
O12 Mo1 O10 Mo4 -61.3(4) . . . 2_566 ?
O5 Mo1 O10 Mo4 -96.2(2) . . . 2_566 ?
O4 Mo1 O10 Mo4 -20.18(17) 2_566 . . 2_566 ?
Mo2 Mo1 O10 Mo4 -119.0(3) . . . 2_566 ?
O11 Mo1 O12 Mo3 69.8(3) . . . 2_566 ?
O13 Mo1 O12 Mo3 177.3(3) . . . 2_566 ?
O10 Mo1 O12 Mo3 -57.3(5) . . . 2_566 ?
O5 Mo1 O12 Mo3 -23.1(3) . . . 2_566 ?
O4 Mo1 O12 Mo3 -96.1(3) 2_566 . . 2_566 ?
Mo2 Mo1 O12 Mo3 -22.9(3) . . . 2_566 ?
O11 Mo1 O13 Cu1 88.4(9) . . . . ?
O12 Mo1 O13 Cu1 -17.5(10) . . . . ?
O10 Mo1 O13 Cu1 -170.3(9) . . . . ?
O5 Mo1 O13 Cu1 -98.0(10) . . . . ?
O4 Mo1 O13 Cu1 -100.2(9) 2_566 . . . ?
Mo2 Mo1 O13 Cu1 -172.5(7) . . . . ?
N3 Cu1 O13 Mo1 -105.6(10) . . . . ?
N3 Cu1 O13 Mo1 74.4(10) 2_677 . . . ?
O1W Cu1 O13 Mo1 165.7(10) . . . . ?
O1W Cu1 O13 Mo1 -14.3(10) 2_677 . . . ?
O13 Cu1 O13 Mo1 -126(100) 2_677 . . . ?
C5 C4 N2 C1 55.4(14) . . . . ?
C5 C4 N2 C3 -115.0(12) . . . . ?
N3 C1 N2 C4 -174.5(10) . . . . ?
N3 C1 N2 C3 -2.0(11) . . . . ?
C2 C3 N2 C4 173.8(11) . . . . ?
C2 C3 N2 C1 2.4(10) . . . . ?
C5 C9 N1 C8 3(2) . . . . ?
C7 C8 N1 C9 0.9(15) . . . . ?
N2 C1 N3 C2 0.8(11) . . . . ?
N2 C1 N3 Cu1 166.4(6) . . . . ?
C3 C2 N3 C1 0.8(11) . . . . ?
C3 C2 N3 Cu1 -163.3(6) . . . . ?
N3 Cu1 N3 C1 -80(100) 2_677 . . . ?
O1W Cu1 N3 C1 -46.2(8) . . . . ?
O1W Cu1 N3 C1 133.8(8) 2_677 . . . ?
O13 Cu1 N3 C1 -130.1(8) . . . . ?
O13 Cu1 N3 C1 49.9(8) 2_677 . . . ?
N3 Cu1 N3 C2 82(100) 2_677 . . . ?
O1W Cu1 N3 C2 116.6(8) . . . . ?
O1W Cu1 N3 C2 -63.4(8) 2_677 . . . ?
O13 Cu1 N3 C2 32.7(8) . . . . ?
O13 Cu1 N3 C2 -147.3(8) 2_677 . . . ?

_diffrn_measured_fraction_theta_max 0.985
_diffrn_reflns_theta_full        25.00
_diffrn_measured_fraction_theta_full 0.985
_refine_diff_density_max         1.956
_refine_diff_density_min         -2.385
_refine_diff_density_rms         0.189

data_3
_database_code_depnum_ccdc_archive 'CCDC 727451'

_audit_creation_method           SHELXL-97
_chemical_name_systematic        
;
?
;
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         'C16 H18 Cu Mo8 N8 O26, 2(H2O)'
_chemical_formula_sum            'C16 H22 Cu Mo8 N8 O28'
_chemical_formula_weight         1605.48

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cu Cu 0.3201 1.2651 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_symmetry_cell_setting           Monoclinic
_symmetry_space_group_name_H-M   'C2/c '

loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y, -z+1/2'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y, z-1/2'
'-x+1/2, -y+1/2, -z'
'x+1/2, -y+1/2, z-1/2'

_cell_length_a                   19.0610(7)
_cell_length_b                   10.4310(7)
_cell_length_c                   18.3960(14)
_cell_angle_alpha                90
_cell_angle_beta                 93.1480(10)
_cell_angle_gamma                90
_cell_volume                     3652.1(4)
_cell_formula_units_Z            4
_cell_measurement_temperature    293(2)
_cell_measurement_reflns_used    'total reflection'
_cell_measurement_theta_min      1.33
_cell_measurement_theta_max      26.04

_exptl_crystal_description       'thin sheet'
_exptl_crystal_colour            'dark green'
_exptl_crystal_size_max          0.45
_exptl_crystal_size_mid          0.36
_exptl_crystal_size_min          0.28
_exptl_crystal_density_meas      ?
_exptl_crystal_density_diffrn    2.920
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             3052
_exptl_absorpt_coefficient_mu    3.334
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_correction_T_min  0.242
_exptl_absorpt_correction_T_max  0.391
_exptl_absorpt_process_details   'SADABS (Sheldrick, 1996)'

_exptl_special_details           
;
?
;

_diffrn_ambient_temperature      293(2)
_diffrn_radiation_wavelength     0.71069
_diffrn_radiation_type           MoK\a
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_monochromator  graphite
_diffrn_measurement_device_type  'Bruker SMART APEX II CCD area-detector'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_detector_area_resol_mean ?
_diffrn_standards_number         0
_diffrn_standards_interval_count ?
_diffrn_standards_interval_time  0
_diffrn_standards_decay_%        ?
_diffrn_reflns_number            8998
_diffrn_reflns_av_R_equivalents  0.0260
_diffrn_reflns_av_sigmaI/netI    0.0273
_diffrn_reflns_limit_h_min       -18
_diffrn_reflns_limit_h_max       22
_diffrn_reflns_limit_k_min       -10
_diffrn_reflns_limit_k_max       12
_diffrn_reflns_limit_l_min       -21
_diffrn_reflns_limit_l_max       21
_diffrn_reflns_theta_min         2.14
_diffrn_reflns_theta_max         25.00
_reflns_number_total             3214
_reflns_number_gt                2930
_reflns_threshold_expression     >2sigma(I)

_computing_data_collection       'Bruker SMART'
_computing_cell_refinement       'Bruker SMART'
_computing_data_reduction        'Bruker SMART'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'

_refine_special_details          
;
Refinement of F² against ALL reflections. The weighted R-factor wR and
goodness of fit S are based on F², conventional R-factors R are based
on F, with F set to zero for negative F². The threshold expression of
F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is
not relevant to the choice of reflections for refinement. R-factors based
on F² are statistically about twice as large as those based on F, and R-
factors based on ALL data will be even larger.

It is difficult to locate hydrogen atoms accurately using X-ray data.
Consequently, it is preferable to calculate the hydrogen positions according to well-established geometrical criteria
and then to adopt a refinement procedure which ensures that a sensible geometry is retained.
The N-H and O-H hydrogens were isotropically refined. The N-H distance(0.85(1) Å) was restrained to be in the vicinity
of corresponding difference Fourier peak. Similarly, the water hydrogens were restrained (O-H = 0.85(1) Å and H...H = 1.38(1) Å) during refinement.
All the donor-acceptor distances are well within the hydrogen bonding interaction range.
;

_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'calc w=1/[σ²(Fo²)+(0.0331P)²+0.2562P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_atom_sites_solution_hydrogens   geom
_refine_ls_hydrogen_treatment    mixed
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       ?
_refine_ls_number_reflns         3214
_refine_ls_number_parameters     288
_refine_ls_number_restraints     4
_refine_ls_R_factor_all          0.0259
_refine_ls_R_factor_gt           0.0228
_refine_ls_wR_factor_ref         0.0615
_refine_ls_wR_factor_gt          0.0601
_refine_ls_goodness_of_fit_ref   1.143
_refine_ls_restrained_S_all      1.142
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Cu1 Cu 0.0000 0.0000 0.0000 0.02014(15) Uani 1 2 d S . .
Mo1 Mo 0.182168(15) 0.03161(3) 0.054734(17) 0.01723(10) Uani 1 1 d . . .
Mo2 Mo 0.254192(16) 0.30003(3) 0.095019(16) 0.01778(10) Uani 1 1 d . . .
Mo3 Mo 0.397287(16) 0.20138(3) 0.028972(17) 0.01985(10) Uani 1 1 d . . .
Mo4 Mo 0.323146(16) -0.07049(3) -0.016513(18) 0.02178(10) Uani 1 1 d . . .
C1 C -0.0395(2) -0.0354(4) 0.1568(2) 0.0291(9) Uani 1 1 d . . .
H1 H -0.0104 -0.1061 0.1651 0.035 Uiso 1 1 calc R . .
C2 C -0.08892(19) 0.1227(3) 0.1044(2) 0.0227(8) Uani 1 1 d . . .
H2 H -0.1026 0.1857 0.0708 0.027 Uiso 1 1 calc R . .
C3 C -0.1636(2) 0.1920(4) 0.2065(2) 0.0294(9) Uani 1 1 d . . .
H3A H -0.1890 0.1408 0.2403 0.035 Uiso 1 1 calc R . .
H3B H -0.1975 0.2280 0.1709 0.035 Uiso 1 1 calc R . .
C4 C -0.1251(2) 0.2996(4) 0.2473(2) 0.0261(9) Uani 1 1 d . . .
C5 C -0.0724(2) 0.2748(4) 0.3009(2) 0.0324(9) Uani 1 1 d . . .
H5 H -0.0607 0.1906 0.3129 0.039 Uiso 1 1 calc R . .
C6 C -0.0376(2) 0.3745(4) 0.3361(2) 0.0375(10) Uani 1 1 d . . .
H6 H -0.0021 0.3577 0.3716 0.045 Uiso 1 1 calc R . .
C7 C -0.0552(2) 0.4973(4) 0.3190(2) 0.0394(11) Uani 1 1 d . . .
H7 H -0.0318 0.5651 0.3424 0.047 Uiso 1 1 calc R . .
C8 C -0.1413(2) 0.4255(4) 0.2322(2) 0.0294(9) Uani 1 1 d . . .
H8 H -0.1766 0.4454 0.1971 0.035 Uiso 1 1 calc R . .
N1 N -0.11398(16) 0.1099(3) 0.16940(17) 0.0250(7) Uani 1 1 d . . .
N2 N -0.08202(18) 0.0070(3) 0.20428(19) 0.0355(8) Uani 1 1 d . . .
N3 N -0.04155(15) 0.0331(3) 0.09403(16) 0.0210(7) Uani 1 1 d . . .
N4 N -0.10629(19) 0.5197(3) 0.2681(2) 0.0345(8) Uani 1 1 d D . .
H1N H -0.117(2) 0.5988(16) 0.262(3) 0.052 Uiso 1 1 d D . .
O1 O 0.22098(13) 0.4519(2) 0.11340(14) 0.0263(6) Uani 1 1 d . . .
O2 O 0.28089(14) 0.2397(3) 0.17708(14) 0.0298(6) Uani 1 1 d . . .
O1W O -0.09977(18) 0.7785(3) 0.29757(19) 0.0463(8) Uani 1 1 d D . .
H1A H -0.129(2) 0.771(4) 0.3305(19) 0.072(19) Uiso 1 1 d D . .
H1B H -0.1127(19) 0.840(3) 0.2696(18) 0.041(14) Uiso 1 1 d D . .
O3 O 0.16437(12) 0.2136(2) 0.07770(13) 0.0193(5) Uani 1 1 d . . .
O4 O 0.34177(11) 0.3533(2) 0.05650(13) 0.0189(5) Uani 1 1 d . . .
O5 O 0.27993(11) 0.1359(2) 0.02841(12) 0.0177(5) Uani 1 1 d . . .
O6 O 0.41716(14) 0.1442(3) 0.11373(15) 0.0329(6) Uani 1 1 d . . .
O7 O 0.47119(13) 0.2787(2) 0.00383(16) 0.0294(6) Uani 1 1 d . . .
O8 O 0.39687(12) 0.0514(2) -0.02808(14) 0.0239(6) Uani 1 1 d . . .
O9 O 0.34359(15) -0.1913(2) -0.07294(17) 0.0389(8) Uani 1 1 d . . .
O10 O 0.34913(14) -0.1218(2) 0.06895(15) 0.0318(6) Uani 1 1 d . . .
O11 O 0.22284(12) -0.0855(2) -0.00775(14) 0.0228(6) Uani 1 1 d . . .
O12 O 0.21236(13) -0.0182(2) 0.13803(14) 0.0256(6) Uani 1 1 d . . .
O13 O 0.09480(12) -0.0172(2) 0.04899(14) 0.0233(6) Uani 1 1 d . . .


_geom_special_details            
;
All esds (except the esd in the dihedral angle between two l.s. planes)
are estimated using the full covariance matrix. The cell esds are taken
into account individually in the estimation of esds in distances, angles
and torsion angles; correlations between esds in cell parameters are only
used when they are defined by crystal symmetry. An approximate (isotropic)
treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Cu1 N3 1.972(3) 5 ?
Cu1 N3 1.972(3) . ?
Cu1 O13 1.983(2) 5 ?
Cu1 O13 1.983(2) . ?
Cu1 O7 2.374(2) 3_445 ?
Cu1 O7 2.374(2) 7 ?
Mo1 O12 1.689(3) . ?
Mo1 O13 1.739(2) . ?
Mo1 O11 1.874(2) . ?
Mo1 O3 1.978(2) . ?
Mo1 O5 2.234(2) . ?
Mo1 O4 2.394(2) 7 ?
Mo1 Mo2 3.1877(4) . ?
Mo2 O2 1.688(3) . ?
Mo2 O1 1.746(2) . ?
Mo2 O4 1.931(2) . ?
Mo2 O3 1.946(2) . ?
Mo2 O5 2.177(2) . ?
Mo2 O5 2.421(2) 7 ?
Mo2 Mo3 3.2154(4) . ?
Mo3 O6 1.693(3) . ?
Mo3 O7 1.709(2) . ?
Mo3 O8 1.883(2) . ?
Mo3 O4 1.987(2) . ?
Mo3 O5 2.338(2) . ?
Mo3 O3 2.401(2) 7 ?
Mo4 O9 1.691(3) . ?
Mo4 O10 1.708(3) . ?
Mo4 O8 1.916(2) . ?
Mo4 O11 1.934(2) . ?
Mo4 O1 2.291(3) 7 ?
Mo4 O5 2.464(2) . ?
C1 N2 1.301(5) . ?
C1 N3 1.357(5) . ?
C1 H1 0.9300 . ?
C2 N1 1.318(5) . ?
C2 N3 1.321(4) . ?
C2 H2 0.9300 . ?
C3 N1 1.470(4) . ?
C3 C4 1.517(5) . ?
C3 H3A 0.9700 . ?
C3 H3B 0.9700 . ?
C4 C8 1.374(5) . ?
C4 C5 1.392(5) . ?
C5 C6 1.376(6) . ?
C5 H5 0.9300 . ?
C6 C7 1.357(6) . ?
C6 H6 0.9300 . ?
C7 N4 1.335(5) . ?
C7 H7 0.9300 . ?
C8 N4 1.340(5) . ?
C8 H8 0.9300 . ?
N1 N2 1.376(4) . ?
N4 H1N 0.856(10) . ?
O1 Mo4 2.291(3) 7 ?
O1W H1A 0.849(10) . ?
O1W H1B 0.850(10) . ?
O3 Mo3 2.401(2) 7 ?
O4 Mo1 2.394(2) 7 ?
O5 Mo2 2.421(2) 7 ?
O7 Cu1 2.374(2) 3 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
N3 Cu1 N3 180.0(2) 5 . ?
N3 Cu1 O13 90.98(11) 5 5 ?
N3 Cu1 O13 89.02(11) . 5 ?
N3 Cu1 O13 89.02(11) 5 . ?
N3 Cu1 O13 90.98(11) . . ?
O13 Cu1 O13 180.00(15) 5 . ?
N3 Cu1 O7 87.73(11) 5 3_445 ?
N3 Cu1 O7 92.27(11) . 3_445 ?
O13 Cu1 O7 83.97(9) 5 3_445 ?
O13 Cu1 O7 96.03(9) . 3_445 ?
N3 Cu1 O7 92.27(11) 5 7 ?
N3 Cu1 O7 87.73(11) . 7 ?
O13 Cu1 O7 96.03(9) 5 7 ?
O13 Cu1 O7 83.97(9) . 7 ?
O7 Cu1 O7 180.0 3_445 7 ?
O12 Mo1 O13 104.04(12) . . ?
O12 Mo1 O11 102.96(12) . . ?
O13 Mo1 O11 101.47(11) . . ?
O12 Mo1 O3 98.92(12) . . ?
O13 Mo1 O3 96.84(11) . . ?
O11 Mo1 O3 146.95(10) . . ?
O12 Mo1 O5 95.72(10) . . ?
O13 Mo1 O5 159.54(10) . . ?
O11 Mo1 O5 78.84(9) . . ?
O3 Mo1 O5 74.56(9) . . ?
O12 Mo1 O4 165.69(10) . 7 ?
O13 Mo1 O4 87.59(10) . 7 ?
O11 Mo1 O4 82.44(10) . 7 ?
O3 Mo1 O4 71.02(9) . 7 ?
O5 Mo1 O4 72.10(8) . 7 ?
O12 Mo1 Mo2 86.45(9) . . ?
O13 Mo1 Mo2 132.07(8) . . ?
O11 Mo1 Mo2 121.86(7) . . ?
O3 Mo1 Mo2 35.33(7) . . ?
O5 Mo1 Mo2 43.02(6) . . ?
O4 Mo1 Mo2 79.51(5) 7 . ?
O2 Mo2 O1 105.07(13) . . ?
O2 Mo2 O4 102.20(11) . . ?
O1 Mo2 O4 98.03(11) . . ?
O2 Mo2 O3 101.12(11) . . ?
O1 Mo2 O3 97.29(11) . . ?
O4 Mo2 O3 147.58(10) . . ?
O2 Mo2 O5 98.27(11) . . ?
O1 Mo2 O5 156.62(11) . . ?
O4 Mo2 O5 78.10(9) . . ?
O3 Mo2 O5 76.52(9) . . ?
O2 Mo2 O5 173.58(11) . 7 ?
O1 Mo2 O5 81.35(10) . 7 ?
O4 Mo2 O5 76.67(9) . 7 ?
O3 Mo2 O5 77.63(9) . 7 ?
O5 Mo2 O5 75.31(9) . 7 ?
O2 Mo2 Mo1 89.15(9) . . ?
O1 Mo2 Mo1 133.30(8) . . ?
O4 Mo2 Mo1 122.53(7) . . ?
O3 Mo2 Mo1 36.01(7) . . ?
O5 Mo2 Mo1 44.43(6) . . ?
O5 Mo2 Mo1 86.23(5) 7 . ?
O2 Mo2 Mo3 89.90(9) . . ?
O1 Mo2 Mo3 133.45(8) . . ?
O4 Mo2 Mo3 35.42(7) . . ?
O3 Mo2 Mo3 123.16(7) . . ?
O5 Mo2 Mo3 46.65(6) . . ?
O5 Mo2 Mo3 85.62(5) 7 . ?
Mo1 Mo2 Mo3 89.684(11) . . ?
O6 Mo3 O7 105.64(13) . . ?
O6 Mo3 O8 102.38(12) . . ?
O7 Mo3 O8 102.68(12) . . ?
O6 Mo3 O4 98.15(12) . . ?
O7 Mo3 O4 98.67(11) . . ?
O8 Mo3 O4 144.94(10) . . ?
O6 Mo3 O5 93.82(11) . . ?
O7 Mo3 O5 159.92(11) . . ?
O8 Mo3 O5 77.31(9) . . ?
O4 Mo3 O5 73.22(8) . . ?
O6 Mo3 O3 163.27(11) . 7 ?
O7 Mo3 O3 88.75(11) . 7 ?
O8 Mo3 O3 82.20(10) . 7 ?
O4 Mo3 O3 70.73(9) . 7 ?
O5 Mo3 O3 71.28(8) . 7 ?
O6 Mo3 Mo2 85.20(9) . . ?
O7 Mo3 Mo2 132.85(9) . . ?
O8 Mo3 Mo2 119.91(7) . . ?
O4 Mo3 Mo2 34.27(6) . . ?
O5 Mo3 Mo2 42.61(6) . . ?
O3 Mo3 Mo2 78.66(6) 7 . ?
O9 Mo4 O10 105.47(14) . . ?
O9 Mo4 O8 103.36(12) . . ?
O10 Mo4 O8 97.63(12) . . ?
O9 Mo4 O11 104.65(12) . . ?
O10 Mo4 O11 97.81(11) . . ?
O8 Mo4 O11 142.91(10) . . ?
O9 Mo4 O1 90.68(12) . 7 ?
O10 Mo4 O1 163.85(11) . 7 ?
O8 Mo4 O1 78.19(10) . 7 ?
O11 Mo4 O1 77.66(10) . 7 ?
O9 Mo4 O5 161.65(12) . . ?
O10 Mo4 O5 92.88(10) . . ?
O8 Mo4 O5 73.62(9) . . ?
O11 Mo4 O5 72.10(9) . . ?
O1 Mo4 O5 70.97(8) 7 . ?
N2 C1 N3 113.7(3) . . ?
N2 C1 H1 123.1 . . ?
N3 C1 H1 123.1 . . ?
N1 C2 N3 110.2(3) . . ?
N1 C2 H2 124.9 . . ?
N3 C2 H2 124.9 . . ?
N1 C3 C4 110.8(3) . . ?
N1 C3 H3A 109.5 . . ?
C4 C3 H3A 109.5 . . ?
N1 C3 H3B 109.5 . . ?
C4 C3 H3B 109.5 . . ?
H3A C3 H3B 108.1 . . ?
C8 C4 C5 117.8(4) . . ?
C8 C4 C3 120.6(4) . . ?
C5 C4 C3 121.6(4) . . ?
C6 C5 C4 120.2(4) . . ?
C6 C5 H5 119.9 . . ?
C4 C5 H5 119.9 . . ?
C7 C6 C5 119.8(4) . . ?
C7 C6 H6 120.1 . . ?
C5 C6 H6 120.1 . . ?
N4 C7 C6 119.3(4) . . ?
N4 C7 H7 120.3 . . ?
C6 C7 H7 120.3 . . ?
N4 C8 C4 120.0(4) . . ?
N4 C8 H8 120.0 . . ?
C4 C8 H8 120.0 . . ?
C2 N1 N2 109.2(3) . . ?
C2 N1 C3 129.5(3) . . ?
N2 N1 C3 121.2(3) . . ?
C1 N2 N1 103.2(3) . . ?
C2 N3 C1 103.7(3) . . ?
C2 N3 Cu1 124.2(3) . . ?
C1 N3 Cu1 131.3(2) . . ?
C7 N4 C8 122.8(4) . . ?
C7 N4 H1N 115(3) . . ?
C8 N4 H1N 122(3) . . ?
Mo2 O1 Mo4 117.44(13) . 7 ?
H1A O1W H1B 108.8(17) . . ?
Mo2 O3 Mo1 108.66(11) . . ?
Mo2 O3 Mo3 110.46(10) . 7 ?
Mo1 O3 Mo3 105.18(10) . 7 ?
Mo2 O4 Mo3 110.31(11) . . ?
Mo2 O4 Mo1 109.27(10) . 7 ?
Mo3 O4 Mo1 105.14(10) . 7 ?
Mo2 O5 Mo1 92.55(8) . . ?
Mo2 O5 Mo3 90.74(8) . . ?
Mo1 O5 Mo3 161.90(11) . . ?
Mo2 O5 Mo2 104.69(9) . 7 ?
Mo1 O5 Mo2 98.82(8) . 7 ?
Mo3 O5 Mo2 97.54(8) . 7 ?
Mo2 O5 Mo4 164.96(11) . . ?
Mo1 O5 Mo4 86.87(7) . . ?
Mo3 O5 Mo4 85.37(7) . . ?
Mo2 O5 Mo4 90.24(8) 7 . ?
Mo3 O7 Cu1 131.48(14) . 3 ?
Mo3 O8 Mo4 118.04(12) . . ?
Mo1 O11 Mo4 116.26(12) . . ?
Mo1 O13 Cu1 147.87(15) . . ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
O12 Mo1 Mo2 O2 -0.46(12) . . . . ?
O13 Mo1 Mo2 O2 105.29(14) . . . . ?
O11 Mo1 Mo2 O2 -103.52(13) . . . . ?
O3 Mo1 Mo2 O2 110.41(16) . . . . ?
O5 Mo1 Mo2 O2 -102.75(12) . . . . ?
O4 Mo1 Mo2 O2 -177.70(11) 7 . . . ?
O12 Mo1 Mo2 O1 -110.53(15) . . . . ?
O13 Mo1 Mo2 O1 -4.79(17) . . . . ?
O11 Mo1 Mo2 O1 146.41(15) . . . . ?
O3 Mo1 Mo2 O1 0.33(17) . . . . ?
O5 Mo1 Mo2 O1 147.18(15) . . . . ?
O4 Mo1 Mo2 O1 72.23(13) 7 . . . ?
O12 Mo1 Mo2 O4 103.50(12) . . . . ?
O13 Mo1 Mo2 O4 -150.76(14) . . . . ?
O11 Mo1 Mo2 O4 0.44(12) . . . . ?
O3 Mo1 Mo2 O4 -145.64(15) . . . . ?
O5 Mo1 Mo2 O4 1.21(12) . . . . ?
O4 Mo1 Mo2 O4 -73.74(11) 7 . . . ?
O12 Mo1 Mo2 O3 -110.87(15) . . . . ?
O13 Mo1 Mo2 O3 -5.12(17) . . . . ?
O11 Mo1 Mo2 O3 146.07(16) . . . . ?
O5 Mo1 Mo2 O3 146.85(15) . . . . ?
O4 Mo1 Mo2 O3 71.89(14) 7 . . . ?
O12 Mo1 Mo2 O5 102.29(12) . . . . ?
O13 Mo1 Mo2 O5 -151.97(15) . . . . ?
O11 Mo1 Mo2 O5 -0.77(12) . . . . ?
O3 Mo1 Mo2 O5 -146.85(15) . . . . ?
O4 Mo1 Mo2 O5 -74.95(10) 7 . . . ?
O12 Mo1 Mo2 O5 175.08(10) . . . 7 ?
O13 Mo1 Mo2 O5 -79.18(12) . . . 7 ?
O11 Mo1 Mo2 O5 72.02(11) . . . 7 ?
O3 Mo1 Mo2 O5 -74.06(13) . . . 7 ?
O5 Mo1 Mo2 O5 72.79(11) . . . 7 ?
O4 Mo1 Mo2 O5 -2.16(7) 7 . . 7 ?
O12 Mo1 Mo2 Mo3 89.44(8) . . . . ?
O13 Mo1 Mo2 Mo3 -164.81(11) . . . . ?
O11 Mo1 Mo2 Mo3 -13.62(9) . . . . ?
O3 Mo1 Mo2 Mo3 -159.69(12) . . . . ?
O5 Mo1 Mo2 Mo3 -12.85(8) . . . . ?
O4 Mo1 Mo2 Mo3 -87.80(6) 7 . . . ?
O2 Mo2 Mo3 O6 0.54(13) . . . . ?
O1 Mo2 Mo3 O6 111.42(15) . . . . ?
O4 Mo2 Mo3 O6 112.08(15) . . . . ?
O3 Mo2 Mo3 O6 -102.71(13) . . . . ?
O5 Mo2 Mo3 O6 -100.96(12) . . . . ?
O5 Mo2 Mo3 O6 -174.85(11) 7 . . . ?
Mo1 Mo2 Mo3 O6 -88.61(9) . . . . ?
O2 Mo2 Mo3 O7 -106.39(16) . . . . ?
O1 Mo2 Mo3 O7 4.49(18) . . . . ?
O4 Mo2 Mo3 O7 5.15(17) . . . . ?
O3 Mo2 Mo3 O7 150.36(16) . . . . ?
O5 Mo2 Mo3 O7 152.11(16) . . . . ?
O5 Mo2 Mo3 O7 78.22(14) 7 . . . ?
Mo1 Mo2 Mo3 O7 164.46(13) . . . . ?
O2 Mo2 Mo3 O8 102.07(13) . . . . ?
O1 Mo2 Mo3 O8 -147.05(15) . . . . ?
O4 Mo2 Mo3 O8 -146.38(15) . . . . ?
O3 Mo2 Mo3 O8 -1.18(12) . . . . ?
O5 Mo2 Mo3 O8 0.57(12) . . . . ?
O5 Mo2 Mo3 O8 -73.32(10) 7 . . . ?
Mo1 Mo2 Mo3 O8 12.93(9) . . . . ?
O2 Mo2 Mo3 O4 -111.54(15) . . . . ?
O1 Mo2 Mo3 O4 -0.66(16) . . . . ?
O3 Mo2 Mo3 O4 145.20(15) . . . . ?
O5 Mo2 Mo3 O4 146.95(15) . . . . ?
O5 Mo2 Mo3 O4 73.06(13) 7 . . . ?
Mo1 Mo2 Mo3 O4 159.31(12) . . . . ?
O2 Mo2 Mo3 O5 101.50(12) . . . . ?
O1 Mo2 Mo3 O5 -147.62(15) . . . . ?
O4 Mo2 Mo3 O5 -146.95(15) . . . . ?
O3 Mo2 Mo3 O5 -1.75(11) . . . . ?
O5 Mo2 Mo3 O5 -73.89(11) 7 . . . ?
Mo1 Mo2 Mo3 O5 12.36(8) . . . . ?
O2 Mo2 Mo3 O3 176.11(11) . . . 7 ?
O1 Mo2 Mo3 O3 -73.01(13) . . . 7 ?
O4 Mo2 Mo3 O3 -72.34(13) . . . 7 ?
O3 Mo2 Mo3 O3 72.86(11) . . . 7 ?
O5 Mo2 Mo3 O3 74.61(10) . . . 7 ?
O5 Mo2 Mo3 O3 0.72(7) 7 . . 7 ?
Mo1 Mo2 Mo3 O3 86.97(5) . . . 7 ?
N1 C3 C4 C8 121.9(4) . . . . ?
N1 C3 C4 C5 -58.0(5) . . . . ?
C8 C4 C5 C6 -1.0(5) . . . . ?
C3 C4 C5 C6 178.9(3) . . . . ?
C4 C5 C6 C7 0.6(6) . . . . ?
C5 C6 C7 N4 0.2(6) . . . . ?
C5 C4 C8 N4 0.7(5) . . . . ?
C3 C4 C8 N4 -179.2(3) . . . . ?
N3 C2 N1 N2 0.0(4) . . . . ?
N3 C2 N1 C3 175.3(3) . . . . ?
C4 C3 N1 C2 -86.8(5) . . . . ?
C4 C3 N1 N2 88.1(4) . . . . ?
N3 C1 N2 N1 0.3(5) . . . . ?
C2 N1 N2 C1 -0.1(4) . . . . ?
C3 N1 N2 C1 -176.0(3) . . . . ?
N1 C2 N3 C1 0.2(4) . . . . ?
N1 C2 N3 Cu1 171.0(2) . . . . ?
N2 C1 N3 C2 -0.3(5) . . . . ?
N2 C1 N3 Cu1 -170.2(3) . . . . ?
N3 Cu1 N3 C2 112(32) 5 . . . ?
O13 Cu1 N3 C2 -43.3(3) 5 . . . ?
O13 Cu1 N3 C2 136.7(3) . . . . ?
O7 Cu1 N3 C2 -127.2(3) 3_445 . . . ?
O7 Cu1 N3 C2 52.8(3) 7 . . . ?
N3 Cu1 N3 C1 -80(32) 5 . . . ?
O13 Cu1 N3 C1 124.8(3) 5 . . . ?
O13 Cu1 N3 C1 -55.2(3) . . . . ?
O7 Cu1 N3 C1 40.9(3) 3_445 . . . ?
O7 Cu1 N3 C1 -139.1(3) 7 . . . ?
C6 C7 N4 C8 -0.5(6) . . . . ?
C4 C8 N4 C7 0.0(6) . . . . ?
O2 Mo2 O1 Mo4 -179.32(12) . . . 7 ?
O4 Mo2 O1 Mo4 75.67(14) . . . 7 ?
O3 Mo2 O1 Mo4 -75.68(14) . . . 7 ?
O5 Mo2 O1 Mo4 -2.9(3) . . . 7 ?
O5 Mo2 O1 Mo4 0.56(11) 7 . . 7 ?
Mo1 Mo2 O1 Mo4 -75.87(15) . . . 7 ?
Mo3 Mo2 O1 Mo4 76.06(16) . . . 7 ?
O2 Mo2 O3 Mo1 -72.76(15) . . . . ?
O1 Mo2 O3 Mo1 -179.76(12) . . . . ?
O4 Mo2 O3 Mo1 62.6(2) . . . . ?
O5 Mo2 O3 Mo1 23.18(11) . . . . ?
O5 Mo2 O3 Mo1 100.80(12) 7 . . . ?
Mo3 Mo2 O3 Mo1 24.49(14) . . . . ?
O2 Mo2 O3 Mo3 172.34(12) . . . 7 ?
O1 Mo2 O3 Mo3 65.35(13) . . . 7 ?
O4 Mo2 O3 Mo3 -52.3(2) . . . 7 ?
O5 Mo2 O3 Mo3 -91.71(11) . . . 7 ?
O5 Mo2 O3 Mo3 -14.09(9) 7 . . 7 ?
Mo1 Mo2 O3 Mo3 -114.90(16) . . . 7 ?
Mo3 Mo2 O3 Mo3 -90.40(9) . . . 7 ?
O12 Mo1 O3 Mo2 70.74(13) . . . . ?
O13 Mo1 O3 Mo2 176.17(12) . . . . ?
O11 Mo1 O3 Mo2 -60.4(2) . . . . ?
O5 Mo1 O3 Mo2 -22.77(11) . . . . ?
O4 Mo1 O3 Mo2 -98.76(12) 7 . . . ?
O12 Mo1 O3 Mo3 -170.97(10) . . . 7 ?
O13 Mo1 O3 Mo3 -65.54(12) . . . 7 ?
O11 Mo1 O3 Mo3 57.9(2) . . . 7 ?
O5 Mo1 O3 Mo3 95.51(10) . . . 7 ?
O4 Mo1 O3 Mo3 19.53(8) 7 . . 7 ?
Mo2 Mo1 O3 Mo3 118.29(15) . . . 7 ?
O2 Mo2 O4 Mo3 72.11(14) . . . . ?
O1 Mo2 O4 Mo3 179.51(12) . . . . ?
O3 Mo2 O4 Mo3 -63.0(2) . . . . ?
O5 Mo2 O4 Mo3 -23.91(11) . . . . ?
O5 Mo2 O4 Mo3 -101.41(12) 7 . . . ?
Mo1 Mo2 O4 Mo3 -24.77(14) . . . . ?
O2 Mo2 O4 Mo1 -172.78(12) . . . 7 ?
O1 Mo2 O4 Mo1 -65.38(13) . . . 7 ?
O3 Mo2 O4 Mo1 52.1(2) . . . 7 ?
O5 Mo2 O4 Mo1 91.20(10) . . . 7 ?
O5 Mo2 O4 Mo1 13.70(9) 7 . . 7 ?
Mo1 Mo2 O4 Mo1 90.34(9) . . . 7 ?
Mo3 Mo2 O4 Mo1 115.11(15) . . . 7 ?
O6 Mo3 O4 Mo2 -68.88(14) . . . . ?
O7 Mo3 O4 Mo2 -176.18(13) . . . . ?
O8 Mo3 O4 Mo2 56.7(2) . . . . ?
O5 Mo3 O4 Mo2 22.68(10) . . . . ?
O3 Mo3 O4 Mo2 98.22(12) 7 . . . ?
O6 Mo3 O4 Mo1 173.44(11) . . . 7 ?
O7 Mo3 O4 Mo1 66.13(12) . . . 7 ?
O8 Mo3 O4 Mo1 -61.02(19) . . . 7 ?
O5 Mo3 O4 Mo1 -95.01(9) . . . 7 ?
O3 Mo3 O4 Mo1 -19.47(8) 7 . . 7 ?
Mo2 Mo3 O4 Mo1 -117.69(14) . . . 7 ?
O2 Mo2 O5 Mo1 80.23(11) . . . . ?
O1 Mo2 O5 Mo1 -96.3(3) . . . . ?
O4 Mo2 O5 Mo1 -178.96(10) . . . . ?
O3 Mo2 O5 Mo1 -19.31(9) . . . . ?
O5 Mo2 O5 Mo1 -99.81(10) 7 . . . ?
Mo3 Mo2 O5 Mo1 162.20(12) . . . . ?
O2 Mo2 O5 Mo3 -81.97(11) . . . . ?
O1 Mo2 O5 Mo3 101.5(2) . . . . ?
O4 Mo2 O5 Mo3 18.84(8) . . . . ?
O3 Mo2 O5 Mo3 178.49(10) . . . . ?
O5 Mo2 O5 Mo3 97.99(9) 7 . . . ?
Mo1 Mo2 O5 Mo3 -162.20(12) . . . . ?
O2 Mo2 O5 Mo2 -179.96(11) . . . 7 ?
O1 Mo2 O5 Mo2 3.5(3) . . . 7 ?
O4 Mo2 O5 Mo2 -79.15(10) . . . 7 ?
O3 Mo2 O5 Mo2 80.50(10) . . . 7 ?
O5 Mo2 O5 Mo2 0.0 7 . . 7 ?
Mo1 Mo2 O5 Mo2 99.81(10) . . . 7 ?
Mo3 Mo2 O5 Mo2 -97.99(9) . . . 7 ?
O2 Mo2 O5 Mo4 -7.2(4) . . . . ?
O1 Mo2 O5 Mo4 176.3(3) . . . . ?
O4 Mo2 O5 Mo4 93.6(4) . . . . ?
O3 Mo2 O5 Mo4 -106.7(4) . . . . ?
O5 Mo2 O5 Mo4 172.7(5) 7 . . . ?
Mo1 Mo2 O5 Mo4 -87.4(4) . . . . ?
Mo3 Mo2 O5 Mo4 74.8(4) . . . . ?
O12 Mo1 O5 Mo2 -78.55(11) . . . . ?
O13 Mo1 O5 Mo2 86.4(3) . . . . ?
O11 Mo1 O5 Mo2 179.33(11) . . . . ?
O3 Mo1 O5 Mo2 19.15(9) . . . . ?
O4 Mo1 O5 Mo2 93.76(9) 7 . . . ?
O12 Mo1 O5 Mo3 21.7(4) . . . . ?
O13 Mo1 O5 Mo3 -173.3(3) . . . . ?
O11 Mo1 O5 Mo3 -80.4(4) . . . . ?
O3 Mo1 O5 Mo3 119.4(4) . . . . ?
O4 Mo1 O5 Mo3 -166.0(4) 7 . . . ?
Mo2 Mo1 O5 Mo3 100.3(4) . . . . ?
O12 Mo1 O5 Mo2 176.16(10) . . . 7 ?
O13 Mo1 O5 Mo2 -18.9(3) . . . 7 ?
O11 Mo1 O5 Mo2 74.03(10) . . . 7 ?
O3 Mo1 O5 Mo2 -86.14(10) . . . 7 ?
O4 Mo1 O5 Mo2 -11.54(7) 7 . . 7 ?
Mo2 Mo1 O5 Mo2 -105.30(10) . . . 7 ?
O12 Mo1 O5 Mo4 86.40(10) . . . . ?
O13 Mo1 O5 Mo4 -108.6(3) . . . . ?
O11 Mo1 O5 Mo4 -15.72(9) . . . . ?
O3 Mo1 O5 Mo4 -175.90(10) . . . . ?
O4 Mo1 O5 Mo4 -101.29(8) 7 . . . ?
Mo2 Mo1 O5 Mo4 164.95(11) . . . . ?
O6 Mo3 O5 Mo2 78.66(11) . . . . ?
O7 Mo3 O5 Mo2 -87.2(3) . . . . ?
O8 Mo3 O5 Mo2 -179.49(10) . . . . ?
O4 Mo3 O5 Mo2 -18.71(9) . . . . ?
O3 Mo3 O5 Mo2 -93.54(9) 7 . . . ?
O6 Mo3 O5 Mo1 -21.9(4) . . . . ?
O7 Mo3 O5 Mo1 172.2(3) . . . . ?
O8 Mo3 O5 Mo1 80.0(4) . . . . ?
O4 Mo3 O5 Mo1 -119.3(4) . . . . ?
O3 Mo3 O5 Mo1 165.9(4) 7 . . . ?
Mo2 Mo3 O5 Mo1 -100.6(4) . . . . ?
O6 Mo3 O5 Mo2 -176.41(11) . . . 7 ?
O7 Mo3 O5 Mo2 17.7(3) . . . 7 ?
O8 Mo3 O5 Mo2 -74.57(10) . . . 7 ?
O4 Mo3 O5 Mo2 86.22(9) . . . 7 ?
O3 Mo3 O5 Mo2 11.39(7) 7 . . 7 ?
Mo2 Mo3 O5 Mo2 104.92(10) . . . 7 ?
O6 Mo3 O5 Mo4 -86.79(11) . . . . ?
O7 Mo3 O5 Mo4 107.3(3) . . . . ?
O8 Mo3 O5 Mo4 15.06(9) . . . . ?
O4 Mo3 O5 Mo4 175.84(9) . . . . ?
O3 Mo3 O5 Mo4 101.01(8) 7 . . . ?
Mo2 Mo3 O5 Mo4 -165.45(11) . . . . ?
O9 Mo4 O5 Mo2 -173.5(4) . . . . ?
O10 Mo4 O5 Mo2 6.6(4) . . . . ?
O8 Mo4 O5 Mo2 -90.5(4) . . . . ?
O11 Mo4 O5 Mo2 103.9(4) . . . . ?
O1 Mo4 O5 Mo2 -173.4(4) 7 . . . ?
O9 Mo4 O5 Mo1 98.3(3) . . . . ?
O10 Mo4 O5 Mo1 -81.57(10) . . . . ?
O8 Mo4 O5 Mo1 -178.68(11) . . . . ?
O11 Mo4 O5 Mo1 15.71(9) . . . . ?
O1 Mo4 O5 Mo1 98.46(9) 7 . . . ?
O9 Mo4 O5 Mo3 -98.1(3) . . . . ?
O10 Mo4 O5 Mo3 82.06(10) . . . . ?
O8 Mo4 O5 Mo3 -15.05(9) . . . . ?
O11 Mo4 O5 Mo3 179.34(10) . . . . ?
O1 Mo4 O5 Mo3 -97.91(9) 7 . . . ?
O9 Mo4 O5 Mo2 -0.6(4) . . . 7 ?
O10 Mo4 O5 Mo2 179.60(10) . . . 7 ?
O8 Mo4 O5 Mo2 82.49(10) . . . 7 ?
O11 Mo4 O5 Mo2 -83.12(10) . . . 7 ?
O1 Mo4 O5 Mo2 -0.37(7) 7 . . 7 ?
O6 Mo3 O7 Cu1 -102.1(2) . . . 3 ?
O8 Mo3 O7 Cu1 150.99(17) . . . 3 ?
O4 Mo3 O7 Cu1 -1.0(2) . . . 3 ?
O5 Mo3 O7 Cu1 63.3(4) . . . 3 ?
O3 Mo3 O7 Cu1 69.27(18) 7 . . 3 ?
Mo2 Mo3 O7 Cu1 -4.0(3) . . . 3 ?
O6 Mo3 O8 Mo4 69.01(16) . . . . ?
O7 Mo3 O8 Mo4 178.43(14) . . . . ?
O4 Mo3 O8 Mo4 -55.4(2) . . . . ?
O5 Mo3 O8 Mo4 -22.17(13) . . . . ?
O3 Mo3 O8 Mo4 -94.64(14) 7 . . . ?
Mo2 Mo3 O8 Mo4 -22.56(17) . . . . ?
O9 Mo4 O8 Mo3 -177.39(15) . . . . ?
O10 Mo4 O8 Mo3 -69.42(16) . . . . ?
O11 Mo4 O8 Mo3 44.4(2) . . . . ?
O1 Mo4 O8 Mo3 94.75(14) 7 . . . ?
O5 Mo4 O8 Mo3 21.35(12) . . . . ?
O12 Mo1 O11 Mo4 -70.77(15) . . . . ?
O13 Mo1 O11 Mo4 -178.27(13) . . . . ?
O3 Mo1 O11 Mo4 59.4(3) . . . . ?
O5 Mo1 O11 Mo4 22.60(12) . . . . ?
O4 Mo1 O11 Mo4 95.76(13) 7 . . . ?
Mo2 Mo1 O11 Mo4 23.14(17) . . . . ?
O9 Mo4 O11 Mo1 177.78(14) . . . . ?
O10 Mo4 O11 Mo1 69.47(16) . . . . ?
O8 Mo4 O11 Mo1 -44.3(2) . . . . ?
O1 Mo4 O11 Mo1 -94.78(14) 7 . . . ?
O5 Mo4 O11 Mo1 -21.05(12) . . . . ?
O12 Mo1 O13 Cu1 162.3(3) . . . . ?
O11 Mo1 O13 Cu1 -91.0(3) . . . . ?
O3 Mo1 O13 Cu1 61.3(3) . . . . ?
O5 Mo1 O13 Cu1 -2.2(5) . . . . ?
O4 Mo1 O13 Cu1 -9.2(3) 7 . . . ?
Mo2 Mo1 O13 Cu1 64.3(3) . . . . ?
N3 Cu1 O13 Mo1 54.3(3) 5 . . . ?
N3 Cu1 O13 Mo1 -125.7(3) . . . . ?
O13 Cu1 O13 Mo1 -66(50) 5 . . . ?
O7 Cu1 O13 Mo1 141.9(3) 3_445 . . . ?
O7 Cu1 O13 Mo1 -38.1(3) 7 . . . ?

loop_
_geom_hbond_atom_site_label_D
_geom_hbond_atom_site_label_H
_geom_hbond_atom_site_label_A
_geom_hbond_distance_DH
_geom_hbond_distance_HA
_geom_hbond_distance_DA
_geom_hbond_angle_DHA
_geom_hbond_site_symmetry_A
N4 H1N O1W 0.856(10) 2.01(3) 2.755(5) 145(4) .
O1W H1B N2 0.850(10) 2.21(2) 2.968(5) 148(4) 1_565
O1W H1A O9 0.849(10) 2.05(2) 2.819(5) 150(4) 8_456

_diffrn_measured_fraction_theta_max 1.000
_diffrn_reflns_theta_full        25.00
_diffrn_measured_fraction_theta_full 1.000
_refine_diff_density_max         0.769
_refine_diff_density_min         -0.950
_refine_diff_density_rms         0.358

data_5
_database_code_depnum_ccdc_archive 'CCDC 727452'

_audit_creation_method           SHELXL-97
_chemical_name_systematic        
;
?
;
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         'C16 H16 Cl Cu3 Mo4 N8 O13'
_chemical_formula_sum            'C16 H16 Cl Cu3 Mo4 N8 O13'
_chemical_formula_weight         1138.20

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cu Cu 0.3201 1.2651 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cl Cl 0.1484 0.1585 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_symmetry_cell_setting           triclinic
_symmetry_space_group_name_H-M   p-1

loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, -z'

_cell_length_a                   10.651(3)
_cell_length_b                   11.293(3)
_cell_length_c                   12.834(7)
_cell_angle_alpha                96.116(3)
_cell_angle_beta                 102.112(3)
_cell_angle_gamma                108.448(4)
_cell_volume                     1406.7(9)
_cell_formula_units_Z            2
_cell_measurement_temperature    293(2)
_cell_measurement_reflns_used    'total reflection'
_cell_measurement_theta_min      1.33
_cell_measurement_theta_max      26.04

_exptl_crystal_description       block
_exptl_crystal_colour            red
_exptl_crystal_size_max          0.4
_exptl_crystal_size_mid          0.36
_exptl_crystal_size_min          0.28
_exptl_crystal_density_meas      ?
_exptl_crystal_density_diffrn    2.687
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             1088
_exptl_absorpt_coefficient_mu    4.122
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_correction_T_min  0.208
_exptl_absorpt_correction_T_max  0.316
_exptl_absorpt_process_details   'SADABS (Sheldrick, 1996)'

_exptl_special_details           
;
?
;

_diffrn_ambient_temperature      293(2)
_diffrn_radiation_wavelength     0.71069
_diffrn_radiation_type           MoK\a
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_monochromator  graphite
_diffrn_measurement_device_type  'Bruker SMART APEX II CCD area-detector'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_detector_area_resol_mean ?
_diffrn_standards_number         0
_diffrn_standards_interval_count ?
_diffrn_standards_interval_time  0
_diffrn_standards_decay_%        ?
_diffrn_reflns_number            6985
_diffrn_reflns_av_R_equivalents  0.0177
_diffrn_reflns_av_sigmaI/netI    0.0408
_diffrn_reflns_limit_h_min       -12
_diffrn_reflns_limit_h_max       9
_diffrn_reflns_limit_k_min       -8
_diffrn_reflns_limit_k_max       13
_diffrn_reflns_limit_l_min       -15
_diffrn_reflns_limit_l_max       14
_diffrn_reflns_theta_min         1.65
_diffrn_reflns_theta_max         25.00
_reflns_number_total             4852
_reflns_number_gt                3917
_reflns_threshold_expression     >2sigma(I)

_computing_data_collection       'Bruker SMART'
_computing_cell_refinement       'Bruker SMART'
_computing_data_reduction        'Bruker SMART'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'

_refine_special_details          
;
Refinement of F² against ALL reflections. The weighted R-factor wR and
goodness of fit S are based on F², conventional R-factors R are based
on F, with F set to zero for negative F². The threshold expression of
F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is
not relevant to the choice of reflections for refinement. R-factors based
on F² are statistically about twice as large as those based on F, and R-
factors based on ALL data will be even larger.
;

_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'calc w=1/[σ²(Fo²)+(0.1125P)²+12.3739P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_atom_sites_solution_hydrogens   geom
_refine_ls_hydrogen_treatment    constr
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       ?
_refine_ls_number_reflns         4852
_refine_ls_number_parameters     406
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0743
_refine_ls_R_factor_gt           0.0615
_refine_ls_wR_factor_ref         0.1887
_refine_ls_wR_factor_gt          0.1768
_refine_ls_goodness_of_fit_ref   1.072
_refine_ls_restrained_S_all      1.072
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Cu1 Cu -0.3378(2) 1.32158(19) 1.48890(15) 0.0697(6) Uani 1 1 d . . .
Cu2 Cu -0.3775(3) 1.4927(3) 1.0778(2) 0.1025(9) Uani 1 1 d . . .
Cu3 Cu 0.12105(16) 1.13291(15) 1.01694(13) 0.0452(4) Uani 1 1 d . . .
Mo1 Mo 0.22293(9) 1.28325(9) 0.41920(8) 0.0309(3) Uani 1 1 d . . .
Mo2 Mo 0.16540(8) 0.98922(8) 0.50199(6) 0.0202(2) Uani 1 1 d . . .
Mo3 Mo -0.10028(9) 0.75480(8) 0.36789(7) 0.0270(3) Uani 1 1 d . . .
Mo4 Mo 0.05618(9) 0.95761(8) 0.71557(6) 0.0228(2) Uani 1 1 d . . .
C1 C 0.3150(13) 0.9978(13) 1.0156(10) 0.043(3) Uani 1 1 d . . .
H1 H 0.2907 0.9767 0.9403 0.051 Uiso 1 1 calc R . .
C2 C 0.3179(12) 1.0765(11) 1.1743(9) 0.037(3) Uani 1 1 d . . .
H2 H 0.2995 1.1171 1.2332 0.044 Uiso 1 1 calc R . .
C3 C 0.5119(12) 1.0169(12) 1.2758(10) 0.044(3) Uani 1 1 d . . .
H3A H 0.5028 1.0645 1.3396 0.052 Uiso 1 1 calc R . .
H3B H 0.6047 1.0550 1.2694 0.052 Uiso 1 1 calc R . .
C4 C 0.4860(11) 0.8801(11) 1.2888(9) 0.035(2) Uani 1 1 d . . .
C5 C 0.5211(12) 0.7955(12) 1.2240(10) 0.043(3) Uani 1 1 d . . .
H5 H 0.5616 0.8195 1.1684 0.051 Uiso 1 1 calc R . .
C6 C 0.4932(13) 0.6757(13) 1.2458(11) 0.047(3) Uani 1 1 d . . .
H7 H 0.5177 0.6173 1.2053 0.057 Uiso 1 1 calc R . .
C7 C 0.4312(15) 0.6393(13) 1.3243(11) 0.050(3) Uani 1 1 d . . .
H6 H 0.4111 0.5556 1.3344 0.061 Uiso 1 1 calc R . .
C8 C 0.4235(12) 0.8391(11) 1.3683(9) 0.037(3) Uani 1 1 d . . .
H8 H 0.3981 0.8957 1.4099 0.044 Uiso 1 1 calc R . .
C9 C -0.3771(13) 1.3726(11) 1.2713(11) 0.044(3) Uani 1 1 d . . .
H9 H -0.4701 1.3567 1.2629 0.053 Uiso 1 1 calc R . .
C10 C -0.1738(13) 1.3860(10) 1.3354(9) 0.037(3) Uani 1 1 d . . .
H10 H -0.0947 1.3836 1.3810 0.044 Uiso 1 1 calc R . .
C11 C -0.0733(12) 1.4634(11) 1.1881(10) 0.037(3) Uani 1 1 d . . .
H11A H 0.0135 1.4781 1.2395 0.045 Uiso 1 1 calc R . .
H11B H -0.0737 1.5446 1.1701 0.045 Uiso 1 1 calc R . .
C12 C -0.0844(11) 1.3756(10) 1.0862(9) 0.029(2) Uani 1 1 d . . .
C13 C -0.1584(12) 1.3778(11) 0.9847(10) 0.040(3) Uani 1 1 d . . .
H13 H -0.2104 1.4302 0.9774 0.048 Uiso 1 1 calc R . .
C14 C -0.1552(11) 1.3029(11) 0.8952(9) 0.036(3) Uani 1 1 d . . .
H14 H -0.2071 1.3025 0.8271 0.043 Uiso 1 1 calc R . .
C15 C -0.0759(10) 1.2289(10) 0.9057(8) 0.029(2) Uani 1 1 d . . .
H15 H -0.0733 1.1792 0.8441 0.035 Uiso 1 1 calc R . .
C16 C -0.0058(12) 1.2998(10) 1.0920(9) 0.033(2) Uani 1 1 d . . .
H16 H 0.0466 1.2988 1.1595 0.040 Uiso 1 1 calc R . .
N1 N 0.2521(10) 1.0618(9) 1.0732(7) 0.034(2) Uani 1 1 d . . .
N2 N 0.4123(11) 0.9699(12) 1.0778(8) 0.050(3) Uani 1 1 d . . .
N3 N 0.4166(9) 1.0243(9) 1.1812(8) 0.037(2) Uani 1 1 d . . .
N4 N 0.3975(12) 0.7197(11) 1.3883(8) 0.048(3) Uani 1 1 d . . .
N5 N -0.2973(12) 1.3613(9) 1.3589(8) 0.044(3) Uani 1 1 d . . .
N6 N -0.3145(10) 1.4083(10) 1.1961(8) 0.040(2) Uani 1 1 d . . .
N7 N -0.1844(9) 1.4132(8) 1.2398(7) 0.0293(19) Uani 1 1 d . . .
N8 N -0.0017(10) 1.2260(8) 1.0027(7) 0.032(2) Uani 1 1 d . . .
O1 O 0.1451(10) 1.3894(8) 0.3901(7) 0.053(2) Uani 1 1 d . . .
O2 O 0.3805(9) 1.3456(8) 0.3956(8) 0.048(2) Uani 1 1 d . . .
O3 O -0.2501(7) 0.6877(7) 0.4293(6) 0.0343(17) Uani 1 1 d . . .
O4 O 0.2826(7) 1.1115(7) 0.4640(6) 0.0297(16) Uani 1 1 d . . .
O5 O -0.1759(9) 0.7002(7) 0.2336(6) 0.0391(19) Uani 1 1 d . . .
O6 O 0.1811(7) 1.0751(6) 0.6462(5) 0.0246(14) Uani 1 1 d . . .
O7 O 0.2474(8) 0.8855(7) 0.5303(6) 0.0329(17) Uani 1 1 d . . .
O8 O -0.0042(9) 0.6649(7) 0.4028(7) 0.0405(19) Uani 1 1 d . . .
O9 O 0.0520(7) 0.9074(6) 0.3567(5) 0.0243(14) Uani 1 1 d . . .
O10 O -0.0280(6) 0.8843(6) 0.5338(5) 0.0219(14) Uani 1 1 d . . .
O11 O -0.1238(7) 0.8464(7) 0.7075(6) 0.0300(16) Uani 1 1 d . . .
O12 O 0.1483(8) 0.8617(7) 0.7402(6) 0.0323(16) Uani 1 1 d . . .
O13 O 0.0911(8) 1.0517(8) 0.8375(6) 0.0372(18) Uani 1 1 d . . .
Cl1 Cl -0.3628(5) 1.6136(5) 0.9589(4) 0.0889(14) Uani 1 1 d . . .


_geom_special_details            
;
All esds (except the esd in the dihedral angle between two l.s. planes)
are estimated using the full covariance matrix. The cell esds are taken
into account individually in the estimation of esds in distances, angles
and torsion angles; correlations between esds in cell parameters are only
used when they are defined by crystal symmetry. An approximate (isotropic)
treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Cu1 N5 1.873(10) . ?
Cu1 N4 1.870(10) 2_578 ?
Cu2 N6 1.987(10) . ?
Cu2 Cl1 2.151(6) . ?
Cu2 Cl1 2.559(6) 2_487 ?
Cu2 Cu2 2.997(6) 2_487 ?
Cu3 N1 1.878(9) . ?
Cu3 N8 1.913(9) . ?
Cu3 O13 2.303(7) . ?
Mo1 O1 1.690(8) . ?
Mo1 O2 1.707(8) . ?
Mo1 O3 1.882(8) 2_576 ?
Mo1 O11 1.922(7) 2_576 ?
Mo1 O4 2.315(7) . ?
Mo2 O7 1.694(7) . ?
Mo2 O4 1.735(7) . ?
Mo2 O9 1.942(7) . ?
Mo2 O6 1.943(7) . ?
Mo2 O10 2.174(6) . ?
Mo2 O10 2.361(7) 2_576 ?
Mo2 Mo3 3.1972(13) . ?
Mo2 Mo4 3.2059(18) . ?
Mo3 O8 1.686(8) . ?
Mo3 O5 1.696(7) . ?
Mo3 O3 1.906(8) . ?
Mo3 O9 2.001(7) . ?
Mo3 O10 2.280(6) . ?
Mo3 O6 2.349(6) 2_576 ?
Mo4 O12 1.688(7) . ?
Mo4 O13 1.693(7) . ?
Mo4 O11 1.905(7) . ?
Mo4 O6 1.989(7) . ?
Mo4 O10 2.275(6) . ?
Mo4 O9 2.340(6) 2_576 ?
C1 N2 1.313(15) . ?
C1 N1 1.384(15) . ?
C1 H1 0.9300 . ?
C2 N1 1.304(14) . ?
C2 N3 1.351(14) . ?
C2 H2 0.9300 . ?
C3 N3 1.439(14) . ?
C3 C4 1.516(16) . ?
C3 H3A 0.9700 . ?
C3 H3B 0.9700 . ?
C4 C8 1.373(16) . ?
C4 C5 1.390(17) . ?
C5 C6 1.364(18) . ?
C5 H5 0.9300 . ?
C6 C7 1.348(19) . ?
C6 H7 0.9300 . ?
C7 N4 1.341(17) . ?
C7 H6 0.9300 . ?
C8 N4 1.352(15) . ?
C8 H8 0.9300 . ?
C9 N5 1.304(16) . ?
C9 N6 1.312(15) . ?
C9 H9 0.9300 . ?
C10 N7 1.288(14) . ?
C10 N5 1.360(16) . ?
C10 H10 0.9300 . ?
C11 N7 1.465(13) . ?
C11 C12 1.514(15) . ?
C11 H11A 0.9700 . ?
C11 H11B 0.9700 . ?
C12 C16 1.371(15) . ?
C12 C13 1.380(16) . ?
C13 C14 1.365(17) . ?
C13 H13 0.9300 . ?
C14 C15 1.361(15) . ?
C14 H14 0.9300 . ?
C15 N8 1.336(13) . ?
C15 H15 0.9300 . ?
C16 N8 1.361(14) . ?
C16 H16 0.9300 . ?
N2 N3 1.386(14) . ?
N4 Cu1 1.870(10) 2_578 ?
N6 N7 1.362(13) . ?
O3 Mo1 1.882(8) 2_576 ?
O6 Mo3 2.349(6) 2_576 ?
O9 Mo4 2.340(6) 2_576 ?
O10 Mo2 2.361(6) 2_576 ?
O11 Mo1 1.922(7) 2_576 ?
Cl1 Cu2 2.559(6) 2_487 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
N5 Cu1 N4 173.9(5) . 2_578 ?
N6 Cu2 Cl1 158.1(4) . . ?
N6 Cu2 Cl1 100.3(3) . 2_487 ?
Cl1 Cu2 Cl1 101.50(19) . 2_487 ?
N6 Cu2 Cu2 145.0(4) . 2_487 ?
Cl1 Cu2 Cu2 56.79(16) . 2_487 ?
Cl1 Cu2 Cu2 44.71(14) 2_487 2_487 ?
N1 Cu3 N8 163.5(4) . . ?
N1 Cu3 O13 96.0(3) . . ?
N8 Cu3 O13 100.5(3) . . ?
O1 Mo1 O2 104.9(5) . . ?
O1 Mo1 O3 98.5(4) . 2_576 ?
O2 Mo1 O3 106.5(4) . 2_576 ?
O1 Mo1 O11 98.3(4) . 2_576 ?
O2 Mo1 O11 102.6(4) . 2_576 ?
O3 Mo1 O11 141.1(3) 2_576 2_576 ?
O1 Mo1 O4 167.2(4) . . ?
O2 Mo1 O4 87.9(3) . . ?
O3 Mo1 O4 78.5(3) 2_576 . ?
O11 Mo1 O4 77.3(3) 2_576 . ?
O7 Mo2 O4 104.7(4) . . ?
O7 Mo2 O9 100.6(3) . . ?
O4 Mo2 O9 96.6(3) . . ?
O7 Mo2 O6 101.9(3) . . ?
O4 Mo2 O6 98.5(3) . . ?
O9 Mo2 O6 148.6(3) . . ?
O7 Mo2 O10 98.1(3) . . ?
O4 Mo2 O10 157.2(3) . . ?
O9 Mo2 O10 78.1(3) . . ?
O6 Mo2 O10 77.3(3) . . ?
O7 Mo2 O10 173.1(3) . 2_576 ?
O4 Mo2 O10 82.2(3) . 2_576 ?
O9 Mo2 O10 77.8(2) . 2_576 ?
O6 Mo2 O10 77.2(2) . 2_576 ?
O10 Mo2 O10 75.0(3) . 2_576 ?
O7 Mo2 Mo3 88.9(3) . . ?
O4 Mo2 Mo3 133.1(2) . . ?
O9 Mo2 Mo3 36.5(2) . . ?
O6 Mo2 Mo3 122.7(2) . . ?
O10 Mo2 Mo3 45.46(17) . . ?
O10 Mo2 Mo3 85.94(16) 2_576 . ?
O7 Mo2 Mo4 89.9(3) . . ?
O4 Mo2 Mo4 134.4(2) . . ?
O9 Mo2 Mo4 123.3(2) . . ?
O6 Mo2 Mo4 35.9(2) . . ?
O10 Mo2 Mo4 45.16(17) . . ?
O10 Mo2 Mo4 85.53(16) 2_576 . ?
Mo3 Mo2 Mo4 89.22(4) . . ?
O8 Mo3 O5 105.0(4) . . ?
O8 Mo3 O3 102.2(4) . . ?
O5 Mo3 O3 101.4(4) . . ?
O8 Mo3 O9 97.0(3) . . ?
O5 Mo3 O9 98.4(3) . . ?
O3 Mo3 O9 147.7(3) . . ?
O8 Mo3 O10 95.1(3) . . ?
O5 Mo3 O10 159.5(3) . . ?
O3 Mo3 O10 78.1(3) . . ?
O9 Mo3 O10 74.5(2) . . ?
O8 Mo3 O6 163.8(3) . 2_576 ?
O5 Mo3 O6 88.0(3) . 2_576 ?
O3 Mo3 O6 84.3(3) . 2_576 ?
O9 Mo3 O6 71.1(2) . 2_576 ?
O10 Mo3 O6 71.5(2) . 2_576 ?
O8 Mo3 Mo2 85.2(3) . . ?
O5 Mo3 Mo2 133.6(3) . . ?
O3 Mo3 Mo2 120.9(2) . . ?
O9 Mo3 Mo2 35.22(18) . . ?
O10 Mo3 Mo2 42.81(16) . . ?
O6 Mo3 Mo2 78.83(17) 2_576 . ?
O12 Mo4 O13 104.1(4) . . ?
O12 Mo4 O11 101.5(3) . . ?
O13 Mo4 O11 100.0(4) . . ?
O12 Mo4 O6 97.2(3) . . ?
O13 Mo4 O6 99.9(4) . . ?
O11 Mo4 O6 148.4(3) . . ?
O12 Mo4 O10 97.1(3) . . ?
O13 Mo4 O10 158.6(3) . . ?
O11 Mo4 O10 78.5(3) . . ?
O6 Mo4 O10 74.0(3) . . ?
O12 Mo4 O9 166.0(3) . 2_576 ?
O13 Mo4 O9 86.4(3) . 2_576 ?
O11 Mo4 O9 85.5(3) . 2_576 ?
O6 Mo4 O9 71.5(2) . 2_576 ?
O10 Mo4 O9 72.2(2) . 2_576 ?
O12 Mo4 Mo2 86.5(3) . . ?
O13 Mo4 Mo2 134.9(3) . . ?
O11 Mo4 Mo2 121.1(2) . . ?
O6 Mo4 Mo2 34.92(18) . . ?
O10 Mo4 Mo2 42.65(16) . . ?
O9 Mo4 Mo2 79.58(16) 2_576 . ?
N2 C1 N1 113.4(10) . . ?
N2 C1 H1 123.3 . . ?
N1 C1 H1 123.3 . . ?
N1 C2 N3 110.2(10) . . ?
N1 C2 H2 124.9 . . ?
N3 C2 H2 124.9 . . ?
N3 C3 C4 110.9(9) . . ?
N3 C3 H3A 109.5 . . ?
C4 C3 H3A 109.5 . . ?
N3 C3 H3B 109.5 . . ?
C4 C3 H3B 109.5 . . ?
H3A C3 H3B 108.1 . . ?
C8 C4 C5 119.3(11) . . ?
C8 C4 C3 117.5(11) . . ?
C5 C4 C3 123.1(11) . . ?
C6 C5 C4 116.8(11) . . ?
C6 C5 H5 121.6 . . ?
C4 C5 H5 121.6 . . ?
C7 C6 C5 121.9(12) . . ?
C7 C6 H7 119.0 . . ?
C5 C6 H7 119.0 . . ?
N4 C7 C6 122.2(12) . . ?
N4 C7 H6 118.9 . . ?
C6 C7 H6 118.9 . . ?
N4 C8 C4 122.6(11) . . ?
N4 C8 H8 118.7 . . ?
C4 C8 H8 118.7 . . ?
N5 C9 N6 114.1(11) . . ?
N5 C9 H9 122.9 . . ?
N6 C9 H9 122.9 . . ?
N7 C10 N5 108.9(10) . . ?
N7 C10 H10 125.5 . . ?
N5 C10 H10 125.5 . . ?
N7 C11 C12 113.2(9) . . ?
N7 C11 H11A 108.9 . . ?
C12 C11 H11A 108.9 . . ?
N7 C11 H11B 108.9 . . ?
C12 C11 H11B 108.9 . . ?
H11A C11 H11B 107.7 . . ?
C16 C12 C13 117.6(10) . . ?
C16 C12 C11 118.9(10) . . ?
C13 C12 C11 123.2(10) . . ?
C14 C13 C12 120.0(11) . . ?
C14 C13 H13 120.0 . . ?
C12 C13 H13 120.0 . . ?
C13 C14 C15 119.9(11) . . ?
C13 C14 H14 120.0 . . ?
C15 C14 H14 120.0 . . ?
N8 C15 C14 121.4(10) . . ?
N8 C15 H15 119.3 . . ?
C14 C15 H15 119.3 . . ?
N8 C16 C12 122.4(10) . . ?
N8 C16 H16 118.8 . . ?
C12 C16 H16 118.8 . . ?
C2 N1 C1 104.3(9) . . ?
C2 N1 Cu3 127.7(8) . . ?
C1 N1 Cu3 127.4(7) . . ?
C1 N2 N3 103.1(9) . . ?
C2 N3 N2 109.0(9) . . ?
C2 N3 C3 129.3(10) . . ?
N2 N3 C3 121.7(10) . . ?
C7 N4 C8 117.1(11) . . ?
C7 N4 Cu1 122.5(9) . 2_578 ?
C8 N4 Cu1 120.0(9) . 2_578 ?
C9 N5 C10 103.9(10) . . ?
C9 N5 Cu1 129.4(9) . . ?
C10 N5 Cu1 126.7(9) . . ?
C9 N6 N7 102.9(9) . . ?
C9 N6 Cu2 125.9(8) . . ?
N7 N6 Cu2 127.9(7) . . ?
C10 N7 N6 110.0(9) . . ?
C10 N7 C11 127.4(10) . . ?
N6 N7 C11 121.9(9) . . ?
C15 N8 C16 118.6(9) . . ?
C15 N8 Cu3 121.6(7) . . ?
C16 N8 Cu3 119.6(7) . . ?
Mo1 O3 Mo3 119.9(4) 2_576 . ?
Mo2 O4 Mo1 119.0(4) . . ?
Mo2 O6 Mo4 109.2(3) . . ?
Mo2 O6 Mo3 109.5(3) . 2_576 ?
Mo4 O6 Mo3 105.0(3) . 2_576 ?
Mo2 O9 Mo3 108.3(3) . . ?
Mo2 O9 Mo4 109.1(3) . 2_576 ?
Mo3 O9 Mo4 105.0(3) . 2_576 ?
Mo2 O10 Mo4 92.2(2) . . ?
Mo2 O10 Mo3 91.7(2) . . ?
Mo4 O10 Mo3 161.6(3) . . ?
Mo2 O10 Mo2 105.0(3) . 2_576 ?
Mo4 O10 Mo2 97.9(2) . 2_576 ?
Mo3 O10 Mo2 98.4(2) . 2_576 ?
Mo4 O11 Mo1 119.7(4) . 2_576 ?
Mo4 O13 Cu3 166.0(5) . . ?
Cu2 Cl1 Cu2 78.50(19) . 2_487 ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
O7 Mo2 Mo3 O8 -0.3(4) . . . . ?
O4 Mo2 Mo3 O8 108.9(4) . . . . ?
O9 Mo2 Mo3 O8 109.4(4) . . . . ?
O6 Mo2 Mo3 O8 -103.8(4) . . . . ?
O10 Mo2 Mo3 O8 -102.8(4) . . . . ?
O10 Mo2 Mo3 O8 -175.8(3) 2_576 . . . ?
Mo4 Mo2 Mo3 O8 -90.2(3) . . . . ?
O7 Mo2 Mo3 O5 -106.4(4) . . . . ?
O4 Mo2 Mo3 O5 2.8(5) . . . . ?
O9 Mo2 Mo3 O5 3.3(5) . . . . ?
O6 Mo2 Mo3 O5 150.1(4) . . . . ?
O10 Mo2 Mo3 O5 151.1(4) . . . . ?
O10 Mo2 Mo3 O5 78.1(4) 2_576 . . . ?
Mo4 Mo2 Mo3 O5 163.7(4) . . . . ?
O7 Mo2 Mo3 O3 101.0(4) . . . . ?
O4 Mo2 Mo3 O3 -149.8(4) . . . . ?
O9 Mo2 Mo3 O3 -149.3(4) . . . . ?
O6 Mo2 Mo3 O3 -2.5(3) . . . . ?
O10 Mo2 Mo3 O3 -1.5(3) . . . . ?
O10 Mo2 Mo3 O3 -74.5(3) 2_576 . . . ?
Mo4 Mo2 Mo3 O3 11.1(3) . . . . ?
O7 Mo2 Mo3 O9 -109.7(4) . . . . ?
O4 Mo2 Mo3 O9 -0.5(4) . . . . ?
O6 Mo2 Mo3 O9 146.9(4) . . . . ?
O10 Mo2 Mo3 O9 147.8(4) . . . . ?
O10 Mo2 Mo3 O9 74.9(3) 2_576 . . . ?
Mo4 Mo2 Mo3 O9 160.4(3) . . . . ?
O7 Mo2 Mo3 O10 102.5(4) . . . . ?
O4 Mo2 Mo3 O10 -148.3(4) . . . . ?
O9 Mo2 Mo3 O10 -147.8(4) . . . . ?
O6 Mo2 Mo3 O10 -1.0(3) . . . . ?
O10 Mo2 Mo3 O10 -73.0(3) 2_576 . . . ?
Mo4 Mo2 Mo3 O10 12.6(2) . . . . ?
O7 Mo2 Mo3 O6 177.3(3) . . . 2_576 ?
O4 Mo2 Mo3 O6 -73.5(4) . . . 2_576 ?
O9 Mo2 Mo3 O6 -73.0(4) . . . 2_576 ?
O6 Mo2 Mo3 O6 73.8(3) . . . 2_576 ?
O10 Mo2 Mo3 O6 74.8(3) . . . 2_576 ?
O10 Mo2 Mo3 O6 1.8(2) 2_576 . . 2_576 ?
Mo4 Mo2 Mo3 O6 87.40(17) . . . 2_576 ?
O7 Mo2 Mo4 O12 2.8(3) . . . . ?
O4 Mo2 Mo4 O12 -107.8(4) . . . . ?
O9 Mo2 Mo4 O12 105.5(3) . . . . ?
O6 Mo2 Mo4 O12 -108.0(4) . . . . ?
O10 Mo2 Mo4 O12 104.4(4) . . . . ?
O10 Mo2 Mo4 O12 177.7(3) 2_576 . . . ?
Mo3 Mo2 Mo4 O12 91.7(3) . . . . ?
O7 Mo2 Mo4 O13 109.2(4) . . . . ?
O4 Mo2 Mo4 O13 -1.4(5) . . . . ?
O9 Mo2 Mo4 O13 -148.1(4) . . . . ?
O6 Mo2 Mo4 O13 -1.6(5) . . . . ?
O10 Mo2 Mo4 O13 -149.2(4) . . . . ?
O10 Mo2 Mo4 O13 -75.9(4) 2_576 . . . ?
Mo3 Mo2 Mo4 O13 -161.9(4) . . . . ?
O7 Mo2 Mo4 O11 -98.4(4) . . . . ?
O4 Mo2 Mo4 O11 150.9(4) . . . . ?
O9 Mo2 Mo4 O11 4.2(3) . . . . ?
O6 Mo2 Mo4 O11 150.8(4) . . . . ?
O10 Mo2 Mo4 O11 3.1(3) . . . . ?
O10 Mo2 Mo4 O11 76.5(3) 2_576 . . . ?
Mo3 Mo2 Mo4 O11 -9.5(3) . . . . ?
O7 Mo2 Mo4 O6 110.8(4) . . . . ?
O4 Mo2 Mo4 O6 0.2(4) . . . . ?
O9 Mo2 Mo4 O6 -146.5(4) . . . . ?
O10 Mo2 Mo4 O6 -147.6(4) . . . . ?
O10 Mo2 Mo4 O6 -74.3(4) 2_576 . . . ?
Mo3 Mo2 Mo4 O6 -160.3(3) . . . . ?
O7 Mo2 Mo4 O10 -101.6(4) . . . . ?
O4 Mo2 Mo4 O10 147.8(4) . . . . ?
O9 Mo2 Mo4 O10 1.1(3) . . . . ?
O6 Mo2 Mo4 O10 147.6(4) . . . . ?
O10 Mo2 Mo4 O10 73.3(3) 2_576 . . . ?
Mo3 Mo2 Mo4 O10 -12.7(2) . . . . ?
O7 Mo2 Mo4 O9 -176.6(3) . . . 2_576 ?
O4 Mo2 Mo4 O9 72.7(4) . . . 2_576 ?
O9 Mo2 Mo4 O9 -74.0(3) . . . 2_576 ?
O6 Mo2 Mo4 O9 72.6(4) . . . 2_576 ?
O10 Mo2 Mo4 O9 -75.0(3) . . . 2_576 ?
O10 Mo2 Mo4 O9 -1.7(2) 2_576 . . 2_576 ?
Mo3 Mo2 Mo4 O9 -87.73(18) . . . 2_576 ?
N3 C3 C4 C8 -105.2(13) . . . . ?
N3 C3 C4 C5 74.2(14) . . . . ?
C8 C4 C5 C6 -1.5(17) . . . . ?
C3 C4 C5 C6 179.2(11) . . . . ?
C4 C5 C6 C7 1.8(19) . . . . ?
C5 C6 C7 N4 -2(2) . . . . ?
C5 C4 C8 N4 1.8(18) . . . . ?
C3 C4 C8 N4 -178.9(10) . . . . ?
N7 C11 C12 C16 -99.8(12) . . . . ?
N7 C11 C12 C13 87.6(13) . . . . ?
C16 C12 C13 C14 2.1(16) . . . . ?
C11 C12 C13 C14 174.8(10) . . . . ?
C12 C13 C14 C15 -1.8(17) . . . . ?
C13 C14 C15 N8 1.0(17) . . . . ?
C13 C12 C16 N8 -1.6(17) . . . . ?
C11 C12 C16 N8 -174.6(10) . . . . ?
N3 C2 N1 C1 -0.4(13) . . . . ?
N3 C2 N1 Cu3 -171.9(8) . . . . ?
N2 C1 N1 C2 2.1(15) . . . . ?
N2 C1 N1 Cu3 173.7(9) . . . . ?
N8 Cu3 N1 C2 0(2) . . . . ?
O13 Cu3 N1 C2 176.9(10) . . . . ?
N8 Cu3 N1 C1 -169.6(13) . . . . ?
O13 Cu3 N1 C1 7.3(11) . . . . ?
N1 C1 N2 N3 -2.8(15) . . . . ?
N1 C2 N3 N2 -1.3(14) . . . . ?
N1 C2 N3 C3 -179.1(11) . . . . ?
C1 N2 N3 C2 2.5(13) . . . . ?
C1 N2 N3 C3 -179.5(11) . . . . ?
C4 C3 N3 C2 115.2(14) . . . . ?
C4 C3 N3 N2 -62.4(14) . . . . ?
C6 C7 N4 C8 3(2) . . . . ?
C6 C7 N4 Cu1 -169.9(10) . . . 2_578 ?
C4 C8 N4 C7 -2.2(18) . . . . ?
C4 C8 N4 Cu1 170.4(9) . . . 2_578 ?
N6 C9 N5 C10 -3.2(14) . . . . ?
N6 C9 N5 Cu1 176.5(8) . . . . ?
N7 C10 N5 C9 1.7(13) . . . . ?
N7 C10 N5 Cu1 -178.0(7) . . . . ?
N4 Cu1 N5 C9 2(5) 2_578 . . . ?
N4 Cu1 N5 C10 -179(100) 2_578 . . . ?
N5 C9 N6 N7 3.3(14) . . . . ?
N5 C9 N6 Cu2 -157.2(9) . . . . ?
Cl1 Cu2 N6 C9 149.9(10) . . . . ?
Cl1 Cu2 N6 C9 -34.1(11) 2_487 . . . ?
Cu2 Cu2 N6 C9 -35.9(14) 2_487 . . . ?
Cl1 Cu2 N6 N7 -5.8(17) . . . . ?
Cl1 Cu2 N6 N7 170.2(9) 2_487 . . . ?
Cu2 Cu2 N6 N7 168.4(6) 2_487 . . . ?
N5 C10 N7 N6 0.2(12) . . . . ?
N5 C10 N7 C11 170.5(9) . . . . ?
C9 N6 N7 C10 -2.0(12) . . . . ?
Cu2 N6 N7 C10 157.9(8) . . . . ?
C9 N6 N7 C11 -172.9(10) . . . . ?
Cu2 N6 N7 C11 -12.9(14) . . . . ?
C12 C11 N7 C10 118.3(12) . . . . ?
C12 C11 N7 N6 -72.5(13) . . . . ?
C14 C15 N8 C16 -0.4(16) . . . . ?
C14 C15 N8 Cu3 -174.9(8) . . . . ?
C12 C16 N8 C15 0.8(16) . . . . ?
C12 C16 N8 Cu3 175.4(8) . . . . ?
N1 Cu3 N8 C15 177.3(12) . . . . ?
O13 Cu3 N8 C15 0.4(9) . . . . ?
N1 Cu3 N8 C16 3(2) . . . . ?
O13 Cu3 N8 C16 -174.0(8) . . . . ?
O8 Mo3 O3 Mo1 70.3(5) . . . 2_576 ?
O5 Mo3 O3 Mo1 178.6(4) . . . 2_576 ?
O9 Mo3 O3 Mo1 -54.7(8) . . . 2_576 ?
O10 Mo3 O3 Mo1 -22.4(4) . . . 2_576 ?
O6 Mo3 O3 Mo1 -94.6(4) 2_576 . . 2_576 ?
Mo2 Mo3 O3 Mo1 -21.3(5) . . . 2_576 ?
O7 Mo2 O4 Mo1 -178.8(4) . . . . ?
O9 Mo2 O4 Mo1 78.3(4) . . . . ?
O6 Mo2 O4 Mo1 -74.1(4) . . . . ?
O10 Mo2 O4 Mo1 3.2(10) . . . . ?
O10 Mo2 O4 Mo1 1.7(3) 2_576 . . . ?
Mo3 Mo2 O4 Mo1 78.6(4) . . . . ?
Mo4 Mo2 O4 Mo1 -74.2(4) . . . . ?
O1 Mo1 O4 Mo2 -4.9(18) . . . . ?
O2 Mo1 O4 Mo2 -179.8(5) . . . . ?
O3 Mo1 O4 Mo2 72.9(4) 2_576 . . . ?
O11 Mo1 O4 Mo2 -76.3(4) 2_576 . . . ?
O7 Mo2 O6 Mo4 -72.8(4) . . . . ?
O4 Mo2 O6 Mo4 -179.9(3) . . . . ?
O9 Mo2 O6 Mo4 62.1(6) . . . . ?
O10 Mo2 O6 Mo4 22.9(3) . . . . ?
O10 Mo2 O6 Mo4 100.2(3) 2_576 . . . ?
Mo3 Mo2 O6 Mo4 23.6(4) . . . . ?
O7 Mo2 O6 Mo3 172.6(3) . . . 2_576 ?
O4 Mo2 O6 Mo3 65.6(4) . . . 2_576 ?
O9 Mo2 O6 Mo3 -52.4(6) . . . 2_576 ?
O10 Mo2 O6 Mo3 -91.6(3) . . . 2_576 ?
O10 Mo2 O6 Mo3 -14.3(3) 2_576 . . 2_576 ?
Mo3 Mo2 O6 Mo3 -90.9(3) . . . 2_576 ?
Mo4 Mo2 O6 Mo3 -114.5(4) . . . 2_576 ?
O12 Mo4 O6 Mo2 73.1(4) . . . . ?
O13 Mo4 O6 Mo2 178.9(3) . . . . ?
O11 Mo4 O6 Mo2 -52.9(7) . . . . ?
O10 Mo4 O6 Mo2 -22.2(3) . . . . ?
O9 Mo4 O6 Mo2 -98.4(3) 2_576 . . . ?
O12 Mo4 O6 Mo3 -169.4(3) . . . 2_576 ?
O13 Mo4 O6 Mo3 -63.7(4) . . . 2_576 ?
O11 Mo4 O6 Mo3 64.6(6) . . . 2_576 ?
O10 Mo4 O6 Mo3 95.2(3) . . . 2_576 ?
O9 Mo4 O6 Mo3 19.1(2) 2_576 . . 2_576 ?
Mo2 Mo4 O6 Mo3 117.4(4) . . . 2_576 ?
O7 Mo2 O9 Mo3 73.3(4) . . . . ?
O4 Mo2 O9 Mo3 179.7(3) . . . . ?
O6 Mo2 O9 Mo3 -61.9(6) . . . . ?
O10 Mo2 O9 Mo3 -22.8(3) . . . . ?
O10 Mo2 O9 Mo3 -99.9(3) 2_576 . . . ?
Mo4 Mo2 O9 Mo3 -23.6(4) . . . . ?
O7 Mo2 O9 Mo4 -172.9(3) . . . 2_576 ?
O4 Mo2 O9 Mo4 -66.6(3) . . . 2_576 ?
O6 Mo2 O9 Mo4 51.8(6) . . . 2_576 ?
O10 Mo2 O9 Mo4 90.9(3) . . . 2_576 ?
O10 Mo2 O9 Mo4 13.9(3) 2_576 . . 2_576 ?
Mo3 Mo2 O9 Mo4 113.7(4) . . . 2_576 ?
Mo4 Mo2 O9 Mo4 90.1(3) . . . 2_576 ?
O8 Mo3 O9 Mo2 -71.3(4) . . . . ?
O5 Mo3 O9 Mo2 -177.6(3) . . . . ?
O3 Mo3 O9 Mo2 54.9(6) . . . . ?
O10 Mo3 O9 Mo2 22.1(3) . . . . ?
O6 Mo3 O9 Mo2 97.4(3) 2_576 . . . ?
O8 Mo3 O9 Mo4 172.3(3) . . . 2_576 ?
O5 Mo3 O9 Mo4 66.0(4) . . . 2_576 ?
O3 Mo3 O9 Mo4 -61.5(6) . . . 2_576 ?
O10 Mo3 O9 Mo4 -94.3(3) . . . 2_576 ?
O6 Mo3 O9 Mo4 -19.0(2) 2_576 . . 2_576 ?
Mo2 Mo3 O9 Mo4 -116.4(4) . . . 2_576 ?
O7 Mo2 O10 Mo4 81.7(3) . . . . ?
O4 Mo2 O10 Mo4 -100.3(7) . . . . ?
O9 Mo2 O10 Mo4 -179.1(3) . . . . ?
O6 Mo2 O10 Mo4 -18.8(2) . . . . ?
O10 Mo2 O10 Mo4 -98.7(3) 2_576 . . . ?
Mo3 Mo2 O10 Mo4 162.1(3) . . . . ?
O7 Mo2 O10 Mo3 -80.3(3) . . . . ?
O4 Mo2 O10 Mo3 97.6(7) . . . . ?
O9 Mo2 O10 Mo3 18.9(2) . . . . ?
O6 Mo2 O10 Mo3 179.2(3) . . . . ?
O10 Mo2 O10 Mo3 99.2(3) 2_576 . . . ?
Mo4 Mo2 O10 Mo3 -162.1(3) . . . . ?
O7 Mo2 O10 Mo2 -179.6(3) . . . 2_576 ?
O4 Mo2 O10 Mo2 -1.6(9) . . . 2_576 ?
O9 Mo2 O10 Mo2 -80.3(3) . . . 2_576 ?
O6 Mo2 O10 Mo2 80.0(3) . . . 2_576 ?
O10 Mo2 O10 Mo2 0.0 2_576 . . 2_576 ?
Mo3 Mo2 O10 Mo2 -99.2(3) . . . 2_576 ?
Mo4 Mo2 O10 Mo2 98.7(3) . . . 2_576 ?
O12 Mo4 O10 Mo2 -76.9(3) . . . . ?
O13 Mo4 O10 Mo2 94.7(9) . . . . ?
O11 Mo4 O10 Mo2 -177.3(3) . . . . ?
O6 Mo4 O10 Mo2 18.6(2) . . . . ?
O9 Mo4 O10 Mo2 93.9(3) 2_576 . . . ?
O12 Mo4 O10 Mo3 25.3(10) . . . . ?
O13 Mo4 O10 Mo3 -163.1(10) . . . . ?
O11 Mo4 O10 Mo3 -75.1(10) . . . . ?
O6 Mo4 O10 Mo3 120.8(10) . . . . ?
O9 Mo4 O10 Mo3 -163.9(10) 2_576 . . . ?
Mo2 Mo4 O10 Mo3 102.2(10) . . . . ?
O12 Mo4 O10 Mo2 177.7(3) . . . 2_576 ?
O13 Mo4 O10 Mo2 -10.7(10) . . . 2_576 ?
O11 Mo4 O10 Mo2 77.3(3) . . . 2_576 ?
O6 Mo4 O10 Mo2 -86.8(3) . . . 2_576 ?
O9 Mo4 O10 Mo2 -11.6(2) 2_576 . . 2_576 ?
Mo2 Mo4 O10 Mo2 -105.4(3) . . . 2_576 ?
O8 Mo3 O10 Mo2 77.3(3) . . . . ?
O5 Mo3 O10 Mo2 -90.6(10) . . . . ?
O3 Mo3 O10 Mo2 178.7(3) . . . . ?
O9 Mo3 O10 Mo2 -18.6(2) . . . . ?
O6 Mo3 O10 Mo2 -93.5(3) 2_576 . . . ?
O8 Mo3 O10 Mo4 -25.0(10) . . . . ?
O5 Mo3 O10 Mo4 167.2(10) . . . . ?
O3 Mo3 O10 Mo4 76.4(10) . . . . ?
O9 Mo3 O10 Mo4 -120.9(10) . . . . ?
O6 Mo3 O10 Mo4 164.3(10) 2_576 . . . ?
Mo2 Mo3 O10 Mo4 -102.3(10) . . . . ?
O8 Mo3 O10 Mo2 -177.3(3) . . . 2_576 ?
O5 Mo3 O10 Mo2 14.8(11) . . . 2_576 ?
O3 Mo3 O10 Mo2 -75.9(3) . . . 2_576 ?
O9 Mo3 O10 Mo2 86.8(3) . . . 2_576 ?
O6 Mo3 O10 Mo2 11.9(2) 2_576 . . 2_576 ?
Mo2 Mo3 O10 Mo2 105.4(3) . . . 2_576 ?
O12 Mo4 O11 Mo1 -75.0(5) . . . 2_576 ?
O13 Mo4 O11 Mo1 178.3(4) . . . 2_576 ?
O6 Mo4 O11 Mo1 50.0(8) . . . 2_576 ?
O10 Mo4 O11 Mo1 20.0(4) . . . 2_576 ?
O9 Mo4 O11 Mo1 92.7(4) 2_576 . . 2_576 ?
Mo2 Mo4 O11 Mo1 17.8(5) . . . 2_576 ?
O12 Mo4 O13 Cu3 -55(2) . . . . ?
O11 Mo4 O13 Cu3 50.1(19) . . . . ?
O6 Mo4 O13 Cu3 -154.6(18) . . . . ?
O10 Mo4 O13 Cu3 134.1(15) . . . . ?
O9 Mo4 O13 Cu3 134.9(19) 2_576 . . . ?
Mo2 Mo4 O13 Cu3 -153.7(17) . . . . ?
N1 Cu3 O13 Mo4 61.7(19) . . . . ?
N8 Cu3 O13 Mo4 -119.2(19) . . . . ?
N6 Cu2 Cl1 Cu2 176.1(10) . . . 2_487 ?
Cl1 Cu2 Cl1 Cu2 0.0 2_487 . . 2_487 ?

_diffrn_measured_fraction_theta_max 0.977
_diffrn_reflns_theta_full        25.00
_diffrn_measured_fraction_theta_full 0.977
_refine_diff_density_max         1.209
_refine_diff_density_min         -3.255
_refine_diff_density_rms         0.234


data_4
_database_code_depnum_ccdc_archive 'CCDC 727453'

_audit_creation_method           SHELXL-97
_chemical_name_systematic        
;
?
;
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         '2(C16 H19 Cu Mo4 N8 O13),3(O)'
_chemical_formula_sum            'C32 H38 Cu2 Mo8 N16 O29'
_chemical_formula_weight         2005.35

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cu Cu 0.3201 1.2651 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_symmetry_cell_setting           Monoclinic
_symmetry_space_group_name_H-M   'C2/c '

loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y, -z+1/2'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y, z-1/2'
'-x+1/2, -y+1/2, -z'
'x+1/2, -y+1/2, z-1/2'

_cell_length_a                   18.456(1)
_cell_length_b                   15.443(1)
_cell_length_c                   20.498(2)
_cell_angle_alpha                90
_cell_angle_beta                 107.187(1)
_cell_angle_gamma                90
_cell_volume                     5581(3)
_cell_formula_units_Z            4
_cell_measurement_temperature    293(2)
_cell_measurement_reflns_used    'total reflection'
_cell_measurement_theta_min      1.33
_cell_measurement_theta_max      26.04

_exptl_crystal_description       block
_exptl_crystal_colour            violate
_exptl_crystal_size_max          0.60
_exptl_crystal_size_mid          0.52
_exptl_crystal_size_min          0.48
_exptl_crystal_density_meas      ?
_exptl_crystal_density_diffrn    2.379
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             3848
_exptl_absorpt_coefficient_mu    2.580
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_correction_T_min  0.230
_exptl_absorpt_correction_T_max  0.292
_exptl_absorpt_process_details   'SADABS (Sheldrick, 1996)'

_exptl_special_details           
;
?
;

_diffrn_ambient_temperature      293(2)
_diffrn_radiation_wavelength     0.71069
_diffrn_radiation_type           MoK\a
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_monochromator  graphite
_diffrn_measurement_device_type  'Bruker SMART APEX II CCD area-detector'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_detector_area_resol_mean ?
_diffrn_standards_number         0
_diffrn_standards_interval_count ?
_diffrn_standards_interval_time  0
_diffrn_standards_decay_%        ?
_diffrn_reflns_number            13814
_diffrn_reflns_av_R_equivalents  0.0219
_diffrn_reflns_av_sigmaI/netI    0.0253
_diffrn_reflns_limit_h_min       -20
_diffrn_reflns_limit_h_max       21
_diffrn_reflns_limit_k_min       -17
_diffrn_reflns_limit_k_max       18
_diffrn_reflns_limit_l_min       -23
_diffrn_reflns_limit_l_max       24
_diffrn_reflns_theta_min         1.75
_diffrn_reflns_theta_max         25.00
_reflns_number_total             4924
_reflns_number_gt                4249
_reflns_threshold_expression     >2sigma(I)

_computing_data_collection       'Bruker SMART'
_computing_cell_refinement       'Bruker SMART'
_computing_data_reduction        'Bruker SMART'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'

_refine_special_details          
;
Refinement of F² against ALL reflections. The weighted R-factor wR and
goodness of fit S are based on F², conventional R-factors R are based
on F, with F set to zero for negative F². The threshold expression of
F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is
not relevant to the choice of reflections for refinement. R-factors based
on F² are statistically about twice as large as those based on F, and R-
factors based on ALL data will be even larger.
;

_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'calc w=1/[σ²(Fo²)+(0.0470P)²+34.7404P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_atom_sites_solution_hydrogens   geom
_refine_ls_hydrogen_treatment    constr
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       ?
_refine_ls_number_reflns         4924
_refine_ls_number_parameters     393
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0366
_refine_ls_R_factor_gt           0.0303
_refine_ls_wR_factor_ref         0.0899
_refine_ls_wR_factor_gt          0.0859
_refine_ls_goodness_of_fit_ref   1.040
_refine_ls_restrained_S_all      1.040
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Cu1 Cu 0.70052(4) -0.00484(4) 0.21728(3) 0.02802(16) Uani 1 1 d . . .
Mo1 Mo 0.83889(2) 0.26026(3) -0.01711(2) 0.02125(12) Uani 1 1 d . . .
Mo2 Mo 0.81071(2) 0.16911(3) 0.13005(2) 0.02372(12) Uani 1 1 d . . .
Mo3 Mo 0.84340(3) 0.03928(3) 0.01592(2) 0.03157(13) Uani 1 1 d . . .
Mo4 Mo 0.80810(3) 0.38589(3) 0.09712(2) 0.02611(12) Uani 1 1 d . . .
C1 C 0.8279(3) 0.0926(3) 0.3099(3) 0.0289(11) Uani 1 1 d . . .
H1 H 0.8614 0.0733 0.2869 0.035 Uiso 1 1 calc R . .
C2 C 0.7836(4) 0.1588(3) 0.3837(3) 0.0358(13) Uani 1 1 d . . .
H2 H 0.7807 0.1929 0.4202 0.043 Uiso 1 1 calc R . .
C3 C 0.9191(3) 0.1879(4) 0.3946(3) 0.0426(15) Uani 1 1 d . . .
H3A H 0.9510 0.1815 0.3649 0.051 Uiso 1 1 calc R . .
H3B H 0.9442 0.1602 0.4379 0.051 Uiso 1 1 calc R . .
C4 C 0.9073(3) 0.2829(3) 0.4061(3) 0.0301(12) Uani 1 1 d . . .
C5 C 0.9341(3) 0.3193(4) 0.4707(3) 0.0360(13) Uani 1 1 d . . .
H5 H 0.9608 0.2859 0.5077 0.043 Uiso 1 1 calc R . .
C6 C 0.9205(4) 0.4057(4) 0.4791(3) 0.0421(15) Uani 1 1 d . . .
H6 H 0.9392 0.4317 0.5218 0.051 Uiso 1 1 calc R . .
C7 C 0.8791(3) 0.4530(3) 0.4242(3) 0.0343(13) Uani 1 1 d . . .
H7 H 0.8680 0.5105 0.4307 0.041 Uiso 1 1 calc R . .
C8 C 0.8684(3) 0.3353(3) 0.3531(3) 0.0322(12) Uani 1 1 d . . .
H8 H 0.8513 0.3115 0.3096 0.039 Uiso 1 1 calc R . .
C9 C 0.6658(3) 0.3880(3) 0.2046(3) 0.0275(11) Uani 1 1 d . . .
H9 H 0.6740 0.3986 0.1627 0.033 Uiso 1 1 calc R . .
C10 C 0.6135(3) 0.3394(3) 0.2811(2) 0.0259(11) Uani 1 1 d . . .
H10 H 0.5812 0.3115 0.3016 0.031 Uiso 1 1 calc R . .
C11 C 0.5466(3) 0.3010(3) 0.1620(3) 0.0298(11) Uani 1 1 d . . .
H11A H 0.5518 0.3126 0.1171 0.036 Uiso 1 1 calc R . .
H11B H 0.4995 0.3270 0.1641 0.036 Uiso 1 1 calc R . .
C12 C 0.5427(3) 0.2053(3) 0.1713(2) 0.0255(11) Uani 1 1 d . . .
C13 C 0.4734(3) 0.1652(3) 0.1599(3) 0.0304(12) Uani 1 1 d . . .
H13 H 0.4288 0.1974 0.1475 0.037 Uiso 1 1 calc R . .
C14 C 0.4713(3) 0.0756(4) 0.1672(3) 0.0354(13) Uani 1 1 d . . .
H14 H 0.4250 0.0474 0.1593 0.043 Uiso 1 1 calc R . .
C15 C 0.5375(3) 0.0293(4) 0.1860(3) 0.0337(12) Uani 1 1 d . . .
H15 H 0.5354 -0.0304 0.1910 0.040 Uiso 1 1 calc R . .
C16 C 0.6075(3) 0.1550(3) 0.1904(2) 0.0252(11) Uani 1 1 d . . .
H16 H 0.6543 0.1821 0.1985 0.030 Uiso 1 1 calc R . .
N1 N 0.7555(2) 0.0708(3) 0.2947(2) 0.0273(9) Uani 1 1 d . . .
N2 N 0.7266(4) 0.1133(3) 0.3421(3) 0.0582(16) Uani 1 1 d . . .
N3 N 0.8454(3) 0.1465(3) 0.3634(2) 0.0338(11) Uani 1 1 d . . .
N4 N 0.6057(2) 0.0680(3) 0.1976(2) 0.0277(9) Uani 1 1 d . . .
N5 N 0.8540(2) 0.4188(3) 0.3613(2) 0.0286(10) Uani 1 1 d . . .
N6 N 0.6098(2) 0.3415(3) 0.2136(2) 0.0265(9) Uani 1 1 d . . .
N7 N 0.7089(2) 0.4177(3) 0.2645(2) 0.0275(9) Uani 1 1 d . . .
N8 N 0.6732(4) 0.3859(4) 0.3099(3) 0.0578(15) Uani 1 1 d . . .
O1 O 0.8929(2) 0.1667(2) -0.01261(18) 0.0297(8) Uani 1 1 d . . .
O2 O 0.8903(2) 0.3383(2) -0.03991(18) 0.0308(8) Uani 1 1 d . . .
O2W O 1.0000 0.3291(6) 0.2500 0.123(4) Uani 1 2 d S . .
O3 O 0.86150(19) 0.2799(2) 0.08083(16) 0.0242(7) Uani 1 1 d . . .
O4 O 0.8593(2) 0.4575(2) 0.06710(19) 0.0387(9) Uani 1 1 d . . .
O5 O 0.8378(2) 0.3976(2) 0.18381(18) 0.0375(9) Uani 1 1 d . . .
O6 O 0.73453(19) 0.2648(2) 0.10626(16) 0.0241(7) Uani 1 1 d . . .
O7 O 0.8655(2) 0.2051(2) 0.20734(18) 0.0360(9) Uani 1 1 d . . .
O8 O 0.75672(18) 0.1625(2) 0.01356(15) 0.0208(7) Uani 1 1 d . . .
O9 O 0.8803(2) 0.0981(2) 0.10297(17) 0.0311(8) Uani 1 1 d . . .
O10 O 0.7860(3) -0.0334(3) 0.0377(2) 0.0448(10) Uani 1 1 d . . .
O11 O 0.7869(2) 0.0562(2) -0.07805(17) 0.0291(8) Uani 1 1 d . . .
O12 O 0.7529(2) 0.0926(2) 0.14884(17) 0.0305(8) Uani 1 1 d . . .
O13 O 0.9194(3) -0.0190(3) 0.0113(2) 0.0548(12) Uani 1 1 d . . .
O1W O 0.9856(4) 0.0143(6) 0.3191(8) 0.247(8) Uani 1 1 d . . .


_geom_special_details            
;
All esds (except the esd in the dihedral angle between two l.s. planes)
are estimated using the full covariance matrix. The cell esds are taken
into account individually in the estimation of esds in distances, angles
and torsion angles; correlations between esds in cell parameters are only
used when they are defined by crystal symmetry. An approximate (isotropic) )
treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Cu1 N1 1.990(4) . ?
Cu1 N7 1.998(4) 4_645 ?
Cu1 N5 2.010(4) 4_645 ?
Cu1 N4 2.019(4) . ?
Mo1 O2 1.683(3) . ?
Mo1 O1 1.742(3) . ?
Mo1 O3 1.950(3) . ?
Mo1 O6 1.965(3) 7_655 ?
Mo1 O8 2.149(3) 7_655 ?
Mo1 O8 2.353(3) . ?
Mo1 Mo4 3.2181(8) . ?
Mo2 O7 1.701(4) . ?
Mo2 O12 1.711(3) . ?
Mo2 O9 1.893(4) . ?
Mo2 O6 1.998(3) . ?
Mo2 O8 2.302(3) . ?
Mo2 O3 2.320(3) . ?
Mo3 O10 1.692(4) . ?
Mo3 O13 1.693(4) . ?
Mo3 O11 1.918(3) . ?
Mo3 O9 1.938(4) . ?
Mo3 O1 2.316(4) . ?
Mo3 O8 2.478(3) . ?
Mo4 O4 1.685(4) . ?
Mo4 O5 1.707(4) . ?
Mo4 O11 1.903(4) 7_655 ?
Mo4 O3 1.989(3) . ?
Mo4 O6 2.351(3) . ?
Mo4 O8 2.352(3) 7_655 ?
C1 N1 1.323(7) . ?
C1 N3 1.338(7) . ?
C1 H1 0.9300 . ?
C2 N3 1.338(7) . ?
C2 N2 1.341(8) . ?
C2 H2 0.9300 . ?
C3 N3 1.468(7) . ?
C3 C4 1.512(7) . ?
C3 H3A 0.9700 . ?
C3 H3B 0.9700 . ?
C4 C8 1.374(7) . ?
C4 C5 1.387(7) . ?
C5 C6 1.379(8) . ?
C5 H5 0.9300 . ?
C6 C7 1.370(8) . ?
C6 H6 0.9300 . ?
C7 N5 1.342(7) . ?
C7 H7 0.9300 . ?
C8 N5 1.338(6) . ?
C8 H8 0.9300 . ?
C9 N6 1.315(6) . ?
C9 N7 1.332(6) . ?
C9 H9 0.9300 . ?
C10 N8 1.302(7) . ?
C10 N6 1.367(6) . ?
C10 H10 0.9300 . ?
C11 N6 1.463(6) . ?
C11 C12 1.495(7) . ?
C11 H11A 0.9700 . ?
C11 H11B 0.9700 . ?
C12 C13 1.377(7) . ?
C12 C16 1.382(7) . ?
C13 C14 1.393(8) . ?
C13 H13 0.9300 . ?
C14 C15 1.370(8) . ?
C14 H14 0.9300 . ?
C15 N4 1.349(7) . ?
C15 H15 0.9300 . ?
C16 N4 1.353(6) . ?
C16 H16 0.9300 . ?
N1 N2 1.402(7) . ?
N5 Cu1 2.010(4) 4_655 ?
N7 N8 1.379(7) . ?
N7 Cu1 1.998(4) 4_655 ?
O6 Mo1 1.965(3) 7_655 ?
O8 Mo1 2.149(3) 7_655 ?
O8 Mo4 2.352(3) 7_655 ?
O11 Mo4 1.903(4) 7_655 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
N1 Cu1 N7 90.07(17) . 4_645 ?
N1 Cu1 N5 179.37(18) . 4_645 ?
N7 Cu1 N5 89.51(17) 4_645 4_645 ?
N1 Cu1 N4 92.27(17) . . ?
N7 Cu1 N4 177.08(17) 4_645 . ?
N5 Cu1 N4 88.16(17) 4_645 . ?
O2 Mo1 O1 104.35(17) . . ?
O2 Mo1 O3 102.00(15) . . ?
O1 Mo1 O3 97.45(15) . . ?
O2 Mo1 O6 99.95(15) . 7_655 ?
O1 Mo1 O6 96.46(15) . 7_655 ?
O3 Mo1 O6 150.13(14) . 7_655 ?
O2 Mo1 O8 98.53(15) . 7_655 ?
O1 Mo1 O8 157.09(14) . 7_655 ?
O3 Mo1 O8 78.86(13) . 7_655 ?
O6 Mo1 O8 78.06(13) 7_655 7_655 ?
O2 Mo1 O8 173.82(15) . . ?
O1 Mo1 O8 81.81(14) . . ?
O3 Mo1 O8 77.50(12) . . ?
O6 Mo1 O8 78.50(12) 7_655 . ?
O8 Mo1 O8 75.31(13) 7_655 . ?
O2 Mo1 Mo4 90.33(12) . . ?
O1 Mo1 Mo4 133.06(12) . . ?
O3 Mo1 Mo4 35.62(10) . . ?
O6 Mo1 Mo4 125.01(10) 7_655 . ?
O8 Mo1 Mo4 46.96(8) 7_655 . ?
O8 Mo1 Mo4 85.76(8) . . ?
O7 Mo2 O12 104.75(17) . . ?
O7 Mo2 O9 101.18(17) . . ?
O12 Mo2 O9 100.86(17) . . ?
O7 Mo2 O6 99.65(16) . . ?
O12 Mo2 O6 97.18(16) . . ?
O9 Mo2 O6 147.83(14) . . ?
O7 Mo2 O8 159.45(15) . . ?
O12 Mo2 O8 95.48(14) . . ?
O9 Mo2 O8 78.09(13) . . ?
O6 Mo2 O8 73.85(12) . . ?
O7 Mo2 O3 87.63(15) . . ?
O12 Mo2 O3 165.11(15) . . ?
O9 Mo2 O3 84.45(14) . . ?
O6 Mo2 O3 72.20(13) . . ?
O8 Mo2 O3 71.83(11) . . ?
O10 Mo3 O13 104.8(2) . . ?
O10 Mo3 O11 99.08(17) . . ?
O13 Mo3 O11 103.28(19) . . ?
O10 Mo3 O9 98.38(17) . . ?
O13 Mo3 O9 103.26(19) . . ?
O11 Mo3 O9 143.11(14) . . ?
O10 Mo3 O1 162.73(17) . . ?
O13 Mo3 O1 92.44(18) . . ?
O11 Mo3 O1 76.63(14) . . ?
O9 Mo3 O1 77.09(14) . . ?
O10 Mo3 O8 93.65(17) . . ?
O13 Mo3 O8 161.52(18) . . ?
O11 Mo3 O8 73.71(12) . . ?
O9 Mo3 O8 72.98(13) . . ?
O1 Mo3 O8 69.08(11) . . ?
O4 Mo4 O5 105.57(19) . . ?
O4 Mo4 O11 101.44(18) . 7_655 ?
O5 Mo4 O11 99.01(17) . 7_655 ?
O4 Mo4 O3 96.89(17) . . ?
O5 Mo4 O3 103.87(16) . . ?
O11 Mo4 O3 145.53(14) 7_655 . ?
O4 Mo4 O6 161.96(15) . . ?
O5 Mo4 O6 90.96(15) . . ?
O11 Mo4 O6 82.63(13) 7_655 . ?
O3 Mo4 O6 71.65(12) . . ?
O4 Mo4 O8 92.10(15) . 7_655 ?
O5 Mo4 O8 162.32(15) . 7_655 ?
O11 Mo4 O8 77.06(13) 7_655 7_655 ?
O3 Mo4 O8 73.29(12) . 7_655 ?
O6 Mo4 O8 71.51(11) . 7_655 ?
O4 Mo4 Mo1 83.77(13) . . ?
O5 Mo4 Mo1 138.59(13) . . ?
O11 Mo4 Mo1 118.94(10) 7_655 . ?
O3 Mo4 Mo1 34.81(9) . . ?
O6 Mo4 Mo1 78.96(8) . . ?
O8 Mo4 Mo1 41.88(8) 7_655 . ?
N1 C1 N3 109.5(5) . . ?
N1 C1 H1 125.2 . . ?
N3 C1 H1 125.2 . . ?
N3 C2 N2 108.0(5) . . ?
N3 C2 H2 126.0 . . ?
N2 C2 H2 126.0 . . ?
N3 C3 C4 109.5(5) . . ?
N3 C3 H3A 109.8 . . ?
C4 C3 H3A 109.8 . . ?
N3 C3 H3B 109.8 . . ?
C4 C3 H3B 109.8 . . ?
H3A C3 H3B 108.2 . . ?
C8 C4 C5 118.1(5) . . ?
C8 C4 C3 120.9(5) . . ?
C5 C4 C3 120.9(5) . . ?
C6 C5 C4 119.1(5) . . ?
C6 C5 H5 120.5 . . ?
C4 C5 H5 120.5 . . ?
C7 C6 C5 119.4(5) . . ?
C7 C6 H6 120.3 . . ?
C5 C6 H6 120.3 . . ?
N5 C7 C6 122.0(5) . . ?
N5 C7 H7 119.0 . . ?
C6 C7 H7 119.0 . . ?
N5 C8 C4 123.0(5) . . ?
N5 C8 H8 118.5 . . ?
C4 C8 H8 118.5 . . ?
N6 C9 N7 109.9(4) . . ?
N6 C9 H9 125.1 . . ?
N7 C9 H9 125.1 . . ?
N8 C10 N6 103.2(4) . . ?
N8 C10 H10 128.4 . . ?
N6 C10 H10 128.4 . . ?
N6 C11 C12 112.9(4) . . ?
N6 C11 H11A 109.0 . . ?
C12 C11 H11A 109.0 . . ?
N6 C11 H11B 109.0 . . ?
C12 C11 H11B 109.0 . . ?
H11A C11 H11B 107.8 . . ?
C13 C12 C16 118.6(5) . . ?
C13 C12 C11 120.0(5) . . ?
C16 C12 C11 121.4(5) . . ?
C12 C13 C14 118.8(5) . . ?
C12 C13 H13 120.6 . . ?
C14 C13 H13 120.6 . . ?
C15 C14 C13 119.9(5) . . ?
C15 C14 H14 120.1 . . ?
C13 C14 H14 120.1 . . ?
N4 C15 C14 121.8(5) . . ?
N4 C15 H15 119.1 . . ?
C14 C15 H15 119.1 . . ?
N4 C16 C12 122.8(5) . . ?
N4 C16 H16 118.6 . . ?
C12 C16 H16 118.6 . . ?
C1 N1 N2 106.4(5) . . ?
C1 N1 Cu1 125.3(3) . . ?
N2 N1 Cu1 128.3(4) . . ?
C2 N2 N1 107.3(5) . . ?
C1 N3 C2 108.8(5) . . ?
C1 N3 C3 126.7(5) . . ?
C2 N3 C3 124.6(5) . . ?
C15 N4 C16 118.2(5) . . ?
C15 N4 Cu1 119.8(3) . . ?
C16 N4 Cu1 121.8(3) . . ?
C8 N5 C7 118.3(4) . . ?
C8 N5 Cu1 122.4(3) . 4_655 ?
C7 N5 Cu1 119.2(3) . 4_655 ?
C9 N6 C10 110.4(4) . . ?
C9 N6 C11 128.7(4) . . ?
C10 N6 C11 120.8(4) . . ?
C9 N7 N8 103.0(4) . . ?
C9 N7 Cu1 128.1(3) . 4_655 ?
N8 N7 Cu1 128.8(4) . 4_655 ?
C10 N8 N7 113.6(5) . . ?
Mo1 O1 Mo3 117.13(17) . . ?
Mo1 O3 Mo4 109.58(16) . . ?
Mo1 O3 Mo2 109.99(14) . . ?
Mo4 O3 Mo2 104.48(14) . . ?
Mo1 O6 Mo2 108.89(15) 7_655 . ?
Mo1 O6 Mo4 109.76(14) 7_655 . ?
Mo2 O6 Mo4 103.08(14) . . ?
Mo1 O8 Mo2 92.78(11) 7_655 . ?
Mo1 O8 Mo4 91.16(11) 7_655 7_655 ?
Mo2 O8 Mo4 162.82(15) . 7_655 ?
Mo1 O8 Mo1 104.69(13) 7_655 . ?
Mo2 O8 Mo1 97.65(12) . . ?
Mo4 O8 Mo1 97.50(11) 7_655 . ?
Mo1 O8 Mo3 163.27(15) 7_655 . ?
Mo2 O8 Mo3 86.25(10) . . ?
Mo4 O8 Mo3 85.19(10) 7_655 . ?
Mo1 O8 Mo3 91.98(11) . . ?
Mo2 O9 Mo3 117.19(18) . . ?
Mo4 O11 Mo3 117.70(17) 7_655 . ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
O2 Mo1 Mo4 O4 1.19(19) . . . . ?
O1 Mo1 Mo4 O4 111.3(2) . . . . ?
O3 Mo1 Mo4 O4 111.6(2) . . . . ?
O6 Mo1 Mo4 O4 -101.23(19) 7_655 . . . ?
O8 Mo1 Mo4 O4 -100.20(18) 7_655 . . . ?
O8 Mo1 Mo4 O4 -174.01(16) . . . . ?
O2 Mo1 Mo4 O5 -105.3(2) . . . . ?
O1 Mo1 Mo4 O5 4.8(3) . . . . ?
O3 Mo1 Mo4 O5 5.1(3) . . . . ?
O6 Mo1 Mo4 O5 152.2(2) 7_655 . . . ?
O8 Mo1 Mo4 O5 153.3(2) 7_655 . . . ?
O8 Mo1 Mo4 O5 79.5(2) . . . . ?
O2 Mo1 Mo4 O11 100.84(17) . . . 7_655 ?
O1 Mo1 Mo4 O11 -149.0(2) . . . 7_655 ?
O3 Mo1 Mo4 O11 -148.7(2) . . . 7_655 ?
O6 Mo1 Mo4 O11 -1.58(17) 7_655 . . 7_655 ?
O8 Mo1 Mo4 O11 -0.55(16) 7_655 . . 7_655 ?
O8 Mo1 Mo4 O11 -74.36(14) . . . 7_655 ?
O2 Mo1 Mo4 O3 -110.4(2) . . . . ?
O1 Mo1 Mo4 O3 -0.3(2) . . . . ?
O6 Mo1 Mo4 O3 147.2(2) 7_655 . . . ?
O8 Mo1 Mo4 O3 148.2(2) 7_655 . . . ?
O8 Mo1 Mo4 O3 74.38(18) . . . . ?
O2 Mo1 Mo4 O6 175.93(15) . . . . ?
O1 Mo1 Mo4 O6 -73.91(18) . . . . ?
O3 Mo1 Mo4 O6 -73.65(18) . . . . ?
O6 Mo1 Mo4 O6 73.51(16) 7_655 . . . ?
O8 Mo1 Mo4 O6 74.54(14) 7_655 . . . ?
O8 Mo1 Mo4 O6 0.73(11) . . . . ?
O2 Mo1 Mo4 O8 101.39(17) . . . 7_655 ?
O1 Mo1 Mo4 O8 -148.45(19) . . . 7_655 ?
O3 Mo1 Mo4 O8 -148.2(2) . . . 7_655 ?
O6 Mo1 Mo4 O8 -1.03(16) 7_655 . . 7_655 ?
O8 Mo1 Mo4 O8 -73.81(15) . . . 7_655 ?
N3 C3 C4 C8 -55.2(7) . . . . ?
N3 C3 C4 C5 123.3(6) . . . . ?
C8 C4 C5 C6 0.2(9) . . . . ?
C3 C4 C5 C6 -178.4(6) . . . . ?
C4 C5 C6 C7 1.9(9) . . . . ?
C5 C6 C7 N5 -3.0(9) . . . . ?
C5 C4 C8 N5 -1.4(8) . . . . ?
C3 C4 C8 N5 177.2(5) . . . . ?
N6 C11 C12 C13 141.3(5) . . . . ?
N6 C11 C12 C16 -39.7(6) . . . . ?
C16 C12 C13 C14 -0.7(7) . . . . ?
C11 C12 C13 C14 178.3(5) . . . . ?
C12 C13 C14 C15 0.5(8) . . . . ?
C13 C14 C15 N4 -0.3(8) . . . . ?
C13 C12 C16 N4 0.6(7) . . . . ?
C11 C12 C16 N4 -178.4(5) . . . . ?
N3 C1 N1 N2 -0.5(6) . . . . ?
N3 C1 N1 Cu1 177.7(3) . . . . ?
N7 Cu1 N1 C1 40.2(4) 4_645 . . . ?
N5 Cu1 N1 C1 -8(17) 4_645 . . . ?
N4 Cu1 N1 C1 -141.5(4) . . . . ?
N7 Cu1 N1 N2 -142.0(4) 4_645 . . . ?
N5 Cu1 N1 N2 170(74) 4_645 . . . ?
N4 Cu1 N1 N2 36.3(4) . . . . ?
N3 C2 N2 N1 0.6(6) . . . . ?
C1 N1 N2 C2 -0.1(6) . . . . ?
Cu1 N1 N2 C2 -178.2(4) . . . . ?
N1 C1 N3 C2 0.9(6) . . . . ?
N1 C1 N3 C3 -177.8(5) . . . . ?
N2 C2 N3 C1 -0.9(6) . . . . ?
N2 C2 N3 C3 177.8(5) . . . . ?
C4 C3 N3 C1 133.6(5) . . . . ?
C4 C3 N3 C2 -44.9(7) . . . . ?
C14 C15 N4 C16 0.2(8) . . . . ?
C14 C15 N4 Cu1 -174.7(4) . . . . ?
C12 C16 N4 C15 -0.4(7) . . . . ?
C12 C16 N4 Cu1 174.4(4) . . . . ?
N1 Cu1 N4 C15 -134.7(4) . . . . ?
N7 Cu1 N4 C15 9(4) 4_645 . . . ?
N5 Cu1 N4 C15 45.8(4) 4_645 . . . ?
N1 Cu1 N4 C16 50.6(4) . . . . ?
N7 Cu1 N4 C16 -166(3) 4_645 . . . ?
N5 Cu1 N4 C16 -128.9(4) 4_645 . . . ?
C4 C8 N5 C7 0.3(8) . . . . ?
C4 C8 N5 Cu1 178.2(4) . . . 4_655 ?
C6 C7 N5 C8 1.9(8) . . . . ?
C6 C7 N5 Cu1 -176.0(5) . . . 4_655 ?
N7 C9 N6 C10 0.6(6) . . . . ?
N7 C9 N6 C11 176.0(5) . . . . ?
N8 C10 N6 C9 -0.1(6) . . . . ?
N8 C10 N6 C11 -175.9(5) . . . . ?
C12 C11 N6 C9 122.3(5) . . . . ?
C12 C11 N6 C10 -62.7(6) . . . . ?
N6 C9 N7 N8 -0.8(6) . . . . ?
N6 C9 N7 Cu1 -177.6(3) . . . 4_655 ?
N6 C10 N8 N7 -0.4(7) . . . . ?
C9 N7 N8 C10 0.8(7) . . . . ?
Cu1 N7 N8 C10 177.5(4) 4_655 . . . ?
O2 Mo1 O1 Mo3 -179.07(18) . . . . ?
O3 Mo1 O1 Mo3 76.47(19) . . . . ?
O6 Mo1 O1 Mo3 -77.03(19) 7_655 . . . ?
O8 Mo1 O1 Mo3 -2.5(5) 7_655 . . . ?
O8 Mo1 O1 Mo3 0.32(16) . . . . ?
Mo4 Mo1 O1 Mo3 76.6(2) . . . . ?
O10 Mo3 O1 Mo1 -0.3(6) . . . . ?
O13 Mo3 O1 Mo1 -179.8(2) . . . . ?
O11 Mo3 O1 Mo1 77.1(2) . . . . ?
O9 Mo3 O1 Mo1 -76.8(2) . . . . ?
O8 Mo3 O1 Mo1 -0.32(16) . . . . ?
O2 Mo1 O3 Mo4 73.35(19) . . . . ?
O1 Mo1 O3 Mo4 179.81(16) . . . . ?
O6 Mo1 O3 Mo4 -63.1(3) 7_655 . . . ?
O8 Mo1 O3 Mo4 -23.11(14) 7_655 . . . ?
O8 Mo1 O3 Mo4 -100.34(16) . . . . ?
O2 Mo1 O3 Mo2 -172.33(16) . . . . ?
O1 Mo1 O3 Mo2 -65.88(18) . . . . ?
O6 Mo1 O3 Mo2 51.2(3) 7_655 . . . ?
O8 Mo1 O3 Mo2 91.20(15) 7_655 . . . ?
O8 Mo1 O3 Mo2 13.97(13) . . . . ?
Mo4 Mo1 O3 Mo2 114.3(2) . . . . ?
O4 Mo4 O3 Mo1 -68.58(19) . . . . ?
O5 Mo4 O3 Mo1 -176.54(17) . . . . ?
O11 Mo4 O3 Mo1 53.3(3) 7_655 . . . ?
O6 Mo4 O3 Mo1 97.11(16) . . . . ?
O8 Mo4 O3 Mo1 21.55(13) 7_655 . . . ?
O4 Mo4 O3 Mo2 173.60(17) . . . . ?
O5 Mo4 O3 Mo2 65.65(18) . . . . ?
O11 Mo4 O3 Mo2 -64.5(3) 7_655 . . . ?
O6 Mo4 O3 Mo2 -20.70(11) . . . . ?
O8 Mo4 O3 Mo2 -96.26(14) 7_655 . . . ?
Mo1 Mo4 O3 Mo2 -117.8(2) . . . . ?
O7 Mo2 O3 Mo1 166.04(19) . . . . ?
O12 Mo2 O3 Mo1 -47.2(6) . . . . ?
O9 Mo2 O3 Mo1 64.57(17) . . . . ?
O6 Mo2 O3 Mo1 -93.03(17) . . . . ?
O8 Mo2 O3 Mo1 -14.69(14) . . . . ?
O7 Mo2 O3 Mo4 -76.43(18) . . . . ?
O12 Mo2 O3 Mo4 70.3(6) . . . . ?
O9 Mo2 O3 Mo4 -177.91(16) . . . . ?
O6 Mo2 O3 Mo4 24.50(14) . . . . ?
O8 Mo2 O3 Mo4 102.84(15) . . . . ?
O7 Mo2 O6 Mo1 -179.56(17) . . . 7_655 ?
O12 Mo2 O6 Mo1 -73.20(18) . . . 7_655 ?
O9 Mo2 O6 Mo1 50.7(3) . . . 7_655 ?
O8 Mo2 O6 Mo1 20.46(13) . . . 7_655 ?
O3 Mo2 O6 Mo1 96.10(16) . . . 7_655 ?
O7 Mo2 O6 Mo4 63.93(17) . . . . ?
O12 Mo2 O6 Mo4 170.30(14) . . . . ?
O9 Mo2 O6 Mo4 -65.9(3) . . . . ?
O8 Mo2 O6 Mo4 -96.05(13) . . . . ?
O3 Mo2 O6 Mo4 -20.41(11) . . . . ?
O4 Mo4 O6 Mo1 -39.5(6) . . . 7_655 ?
O5 Mo4 O6 Mo1 163.89(19) . . . 7_655 ?
O11 Mo4 O6 Mo1 64.93(16) 7_655 . . 7_655 ?
O3 Mo4 O6 Mo1 -91.81(16) . . . 7_655 ?
O8 Mo4 O6 Mo1 -13.84(13) 7_655 . . 7_655 ?
Mo1 Mo4 O6 Mo1 -56.57(12) . . . 7_655 ?
O4 Mo4 O6 Mo2 76.4(6) . . . . ?
O5 Mo4 O6 Mo2 -80.22(17) . . . . ?
O11 Mo4 O6 Mo2 -179.18(15) 7_655 . . . ?
O3 Mo4 O6 Mo2 24.08(13) . . . . ?
O8 Mo4 O6 Mo2 102.05(14) 7_655 . . . ?
Mo1 Mo4 O6 Mo2 59.33(10) . . . . ?
O7 Mo2 O8 Mo1 -91.7(4) . . . 7_655 ?
O12 Mo2 O8 Mo1 78.28(15) . . . 7_655 ?
O9 Mo2 O8 Mo1 178.26(15) . . . 7_655 ?
O6 Mo2 O8 Mo1 -17.62(12) . . . 7_655 ?
O3 Mo2 O8 Mo1 -93.74(13) . . . 7_655 ?
O7 Mo2 O8 Mo4 165.3(5) . . . 7_655 ?
O12 Mo2 O8 Mo4 -24.8(5) . . . 7_655 ?
O9 Mo2 O8 Mo4 75.2(5) . . . 7_655 ?
O6 Mo2 O8 Mo4 -120.7(5) . . . 7_655 ?
O3 Mo2 O8 Mo4 163.2(5) . . . 7_655 ?
O7 Mo2 O8 Mo1 13.6(5) . . . . ?
O12 Mo2 O8 Mo1 -176.48(14) . . . . ?
O9 Mo2 O8 Mo1 -76.51(14) . . . . ?
O6 Mo2 O8 Mo1 87.61(13) . . . . ?
O3 Mo2 O8 Mo1 11.49(11) . . . . ?
O7 Mo2 O8 Mo3 105.1(4) . . . . ?
O12 Mo2 O8 Mo3 -84.98(14) . . . . ?
O9 Mo2 O8 Mo3 14.99(12) . . . . ?
O6 Mo2 O8 Mo3 179.11(13) . . . . ?
O3 Mo2 O8 Mo3 102.99(12) . . . . ?
O2 Mo1 O8 Mo1 -4.4(14) . . . 7_655 ?
O1 Mo1 O8 Mo1 -178.86(16) . . . 7_655 ?
O3 Mo1 O8 Mo1 81.58(14) . . . 7_655 ?
O6 Mo1 O8 Mo1 -80.50(14) 7_655 . . 7_655 ?
O8 Mo1 O8 Mo1 0.0 7_655 . . 7_655 ?
Mo4 Mo1 O8 Mo1 46.52(10) . . . 7_655 ?
O2 Mo1 O8 Mo2 -99.3(13) . . . . ?
O1 Mo1 O8 Mo2 86.22(15) . . . . ?
O3 Mo1 O8 Mo2 -13.34(12) . . . . ?
O6 Mo1 O8 Mo2 -175.42(14) 7_655 . . . ?
O8 Mo1 O8 Mo2 -94.92(14) 7_655 . . . ?
Mo4 Mo1 O8 Mo2 -48.40(9) . . . . ?
O2 Mo1 O8 Mo4 88.8(13) . . . 7_655 ?
O1 Mo1 O8 Mo4 -85.67(15) . . . 7_655 ?
O3 Mo1 O8 Mo4 174.77(14) . . . 7_655 ?
O6 Mo1 O8 Mo4 12.69(12) 7_655 . . 7_655 ?
O8 Mo1 O8 Mo4 93.19(14) 7_655 . . 7_655 ?
Mo4 Mo1 O8 Mo4 139.71(9) . . . 7_655 ?
O2 Mo1 O8 Mo3 174.2(13) . . . . ?
O1 Mo1 O8 Mo3 -0.26(13) . . . . ?
O3 Mo1 O8 Mo3 -99.82(13) . . . . ?
O6 Mo1 O8 Mo3 98.09(12) 7_655 . . . ?
O8 Mo1 O8 Mo3 178.60(17) 7_655 . . . ?
Mo4 Mo1 O8 Mo3 -134.88(8) . . . . ?
O10 Mo3 O8 Mo1 -4.5(5) . . . 7_655 ?
O13 Mo3 O8 Mo1 177.0(6) . . . 7_655 ?
O11 Mo3 O8 Mo1 93.9(5) . . . 7_655 ?
O9 Mo3 O8 Mo1 -102.2(5) . . . 7_655 ?
O1 Mo3 O8 Mo1 175.5(5) . . . 7_655 ?
O10 Mo3 O8 Mo2 82.67(15) . . . . ?
O13 Mo3 O8 Mo2 -95.8(6) . . . . ?
O11 Mo3 O8 Mo2 -178.92(14) . . . . ?
O9 Mo3 O8 Mo2 -14.98(12) . . . . ?
O1 Mo3 O8 Mo2 -97.33(12) . . . . ?
O10 Mo3 O8 Mo4 -82.42(15) . . . 7_655 ?
O13 Mo3 O8 Mo4 99.1(6) . . . 7_655 ?
O11 Mo3 O8 Mo4 15.98(12) . . . 7_655 ?
O9 Mo3 O8 Mo4 179.92(14) . . . 7_655 ?
O1 Mo3 O8 Mo4 97.57(12) . . . 7_655 ?
O10 Mo3 O8 Mo1 -179.78(15) . . . . ?
O13 Mo3 O8 Mo1 1.7(6) . . . . ?
O11 Mo3 O8 Mo1 -81.38(13) . . . . ?
O9 Mo3 O8 Mo1 82.56(13) . . . . ?
O1 Mo3 O8 Mo1 0.21(11) . . . . ?
O7 Mo2 O9 Mo3 179.19(19) . . . . ?
O12 Mo2 O9 Mo3 71.6(2) . . . . ?
O6 Mo2 O9 Mo3 -51.4(4) . . . . ?
O8 Mo2 O9 Mo3 -21.78(17) . . . . ?
O3 Mo2 O9 Mo3 -94.34(19) . . . . ?
O10 Mo3 O9 Mo2 -70.6(2) . . . . ?
O13 Mo3 O9 Mo2 -178.1(2) . . . . ?
O11 Mo3 O9 Mo2 46.9(3) . . . . ?
O1 Mo3 O9 Mo2 92.4(2) . . . . ?
O8 Mo3 O9 Mo2 20.65(16) . . . . ?
O10 Mo3 O11 Mo4 68.6(2) . . . 7_655 ?
O13 Mo3 O11 Mo4 176.3(2) . . . 7_655 ?
O9 Mo3 O11 Mo4 -48.7(3) . . . 7_655 ?
O1 Mo3 O11 Mo4 -94.3(2) . . . 7_655 ?
O8 Mo3 O11 Mo4 -22.52(16) . . . 7_655 ?

_diffrn_measured_fraction_theta_max 0.999
_diffrn_reflns_theta_full        25.00
_diffrn_measured_fraction_theta_full 0.999
_refine_diff_density_max         1.822
_refine_diff_density_min         -0.629
_refine_diff_density_rms         0.124

data_2
_database_code_depnum_ccdc_archive 'CCDC 736016'

_audit_creation_method           SHELXL-97
_chemical_name_systematic        
;
?
;
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         'C18 H18 Cu Mo4 N6 O13'
_chemical_formula_sum            'C18 H18 Cu Mo4 N6 O13'
_chemical_formula_weight         973.68

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cu Cu 0.3201 1.2651 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_symmetry_cell_setting           Monoclinic
_symmetry_space_group_name_H-M   P21/n

loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x-1/2, -y-1/2, z-1/2'

_cell_length_a                   12.3881(17)
_cell_length_b                   15.8284(21)
_cell_length_c                   14.1052(19)
_cell_angle_alpha                90
_cell_angle_beta                 92.2640(24)
_cell_angle_gamma                90
_cell_volume                     2763.5(17)
_cell_formula_units_Z            4
_cell_measurement_temperature    293(2)
_cell_measurement_reflns_used    'total reflection'
_cell_measurement_theta_min      1.33
_cell_measurement_theta_max      25.07

_exptl_crystal_description       block
_exptl_crystal_colour            blue
_exptl_crystal_size_max          0.42
_exptl_crystal_size_mid          0.34
_exptl_crystal_size_min          0.29
_exptl_crystal_density_meas      ?
_exptl_crystal_density_diffrn    2.340
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             1876
_exptl_absorpt_coefficient_mu    2.596
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_correction_T_min  0.359
_exptl_absorpt_correction_T_max  0.470
_exptl_absorpt_process_details   'SADABS (Sheldrick, 1996)'

_exptl_special_details           
;
?
;

_diffrn_ambient_temperature      293(2)
_diffrn_radiation_wavelength     0.71069
_diffrn_radiation_type           MoK\a
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_monochromator  graphite
_diffrn_measurement_device_type  'Bruker SMART APEX II CCD area-detector'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_detector_area_resol_mean ?
_diffrn_standards_number         0
_diffrn_standards_interval_count ?
_diffrn_standards_interval_time  0
_diffrn_standards_decay_%        ?
_diffrn_reflns_number            13357
_diffrn_reflns_av_R_equivalents  0.0518
_diffrn_reflns_av_sigmaI/netI    0.0496
_diffrn_reflns_limit_h_min       -14
_diffrn_reflns_limit_h_max       14
_diffrn_reflns_limit_k_min       -18
_diffrn_reflns_limit_k_max       18
_diffrn_reflns_limit_l_min       -16
_diffrn_reflns_limit_l_max       8
_diffrn_reflns_theta_min         1.93
_diffrn_reflns_theta_max         25.07
_reflns_number_total             4868
_reflns_number_gt                3913
_reflns_threshold_expression     >2sigma(I)

_computing_data_collection       'Bruker SMART'
_computing_cell_refinement       'Bruker SMART'
_computing_data_reduction        'Bruker SMART'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'

_refine_special_details          
;
Refinement of F² against ALL reflections. The weighted R-factor wR and
goodness of fit S are based on F², conventional R-factors R are based
on F, with F set to zero for negative F². The threshold expression of
F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is
not relevant to the choice of reflections for refinement. R-factors based
on F² are statistically about twice as large as those based on F, and R-
factors based on ALL data will be even larger.
;

_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'calc w=1/[σ²(Fo²)+(0.0405P)²+5.5729P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_atom_sites_solution_hydrogens   geom
_refine_ls_hydrogen_treatment    constr
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       ?
_refine_ls_number_reflns         4868
_refine_ls_number_parameters     379
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0531
_refine_ls_R_factor_gt           0.0374
_refine_ls_wR_factor_ref         0.0947
_refine_ls_wR_factor_gt          0.0880
_refine_ls_goodness_of_fit_ref   1.048
_refine_ls_restrained_S_all      1.048
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Cu1 Cu 0.76183(6) 0.14820(4) 0.80851(5) 0.03300(19) Uani 1 1 d . . .
Mo1 Mo 0.45793(4) 0.20204(3) 0.47913(4) 0.03011(14) Uani 1 1 d . . .
Mo2 Mo 0.57736(4) 0.00947(3) 0.61406(4) 0.02801(14) Uani 1 1 d . . .
Mo3 Mo 0.66758(4) 0.11108(3) 0.38114(4) 0.03635(15) Uani 1 1 d . . .
Mo4 Mo 0.26488(4) 0.10535(3) 0.62197(4) 0.03927(16) Uani 1 1 d . . .
C1 C 0.6315(5) 0.2995(3) 0.8493(4) 0.0328(13) Uani 1 1 d . . .
H1 H 0.6930 0.3306 0.8661 0.039 Uiso 1 1 calc R . .
C2 C 0.5256(5) 0.2001(4) 0.8008(4) 0.0392(15) Uani 1 1 d . . .
H2 H 0.5009 0.1482 0.7778 0.047 Uiso 1 1 calc R . .
C3 C 0.4620(5) 0.2666(4) 0.8210(5) 0.0428(15) Uani 1 1 d . . .
H3 H 0.3871 0.2694 0.8148 0.051 Uiso 1 1 calc R . .
C4 C 0.5027(5) 0.4172(3) 0.8746(4) 0.0381(14) Uani 1 1 d . . .
H4A H 0.5515 0.4386 0.9245 0.046 Uiso 1 1 calc R . .
H4B H 0.4298 0.4194 0.8970 0.046 Uiso 1 1 calc R . .
C5 C 0.5105(5) 0.4710(4) 0.7876(5) 0.0364(14) Uani 1 1 d . . .
C6 C 0.4353(5) 0.4635(4) 0.7110(5) 0.0505(18) Uani 1 1 d . . .
H6 H 0.3756 0.4283 0.7152 0.061 Uiso 1 1 calc R . .
C7 C 0.4511(6) 0.5083(4) 0.6310(5) 0.0544(19) Uani 1 1 d . . .
H7 H 0.4036 0.5022 0.5787 0.065 Uiso 1 1 calc R . .
C8 C 0.5366(5) 0.5625(4) 0.6268(5) 0.0462(16) Uani 1 1 d . . .
H8 H 0.5453 0.5941 0.5720 0.055 Uiso 1 1 calc R . .
C9 C 0.5934(5) 0.5260(3) 0.7791(5) 0.0344(14) Uani 1 1 d . . .
H9 H 0.6420 0.5326 0.8304 0.041 Uiso 1 1 calc R . .
C10 C 0.7677(5) 0.2639(4) 0.6438(4) 0.0380(15) Uani 1 1 d . . .
H10 H 0.6926 0.2650 0.6406 0.046 Uiso 1 1 calc R . .
C11 C 0.9311(6) 0.2333(4) 0.6919(6) 0.0556(19) Uani 1 1 d . . .
H11 H 0.9901 0.2115 0.7266 0.067 Uiso 1 1 calc R . .
C12 C 0.9338(6) 0.2854(6) 0.6093(7) 0.079(3) Uani 1 1 d . . .
H12 H 0.9952 0.3032 0.5792 0.095 Uiso 1 1 calc R . .
C13 C 0.7874(6) 0.3510(4) 0.4989(4) 0.0413(15) Uani 1 1 d . . .
H13A H 0.7104 0.3410 0.4906 0.050 Uiso 1 1 calc R . .
H13B H 0.8217 0.3291 0.4434 0.050 Uiso 1 1 calc R . .
C14 C 0.8068(5) 0.4447(4) 0.5048(4) 0.0384(15) Uani 1 1 d . . .
C15 C 0.8403(7) 0.4873(5) 0.4265(6) 0.066(2) Uani 1 1 d . . .
H15 H 0.8554 0.4571 0.3721 0.080 Uiso 1 1 calc R . .
C16 C 0.8513(7) 0.5704(5) 0.4269(6) 0.070(2) Uani 1 1 d . . .
H16 H 0.8799 0.5989 0.3760 0.084 Uiso 1 1 calc R . .
C17 C 0.8199(6) 0.6113(5) 0.5028(5) 0.0569(19) Uani 1 1 d . . .
H17 H 0.8188 0.6700 0.5001 0.068 Uiso 1 1 calc R . .
C18 C 0.7838(5) 0.4900(4) 0.5829(5) 0.0392(15) Uani 1 1 d . . .
H18 H 0.7635 0.4620 0.6374 0.047 Uiso 1 1 calc R . .
O1 O 0.7509(3) 0.1709(3) 0.4519(4) 0.0517(12) Uani 1 1 d . . .
O2 O 0.7139(4) 0.1262(3) 0.2722(4) 0.0556(13) Uani 1 1 d . . .
O3 O 0.5414(3) 0.1803(2) 0.3730(3) 0.0383(10) Uani 1 1 d . . .
O4 O 0.5629(3) 0.0806(2) 0.5123(3) 0.0359(10) Uani 1 1 d . . .
O5 O 0.6391(3) -0.0858(2) 0.5823(3) 0.0354(9) Uani 1 1 d . . .
O6 O 0.6620(3) 0.0577(3) 0.6970(3) 0.0432(11) Uani 1 1 d . . .
O7 O 0.4529(3) -0.0098(2) 0.6675(3) 0.0404(10) Uani 1 1 d . . .
O8 O 0.5410(3) 0.2719(3) 0.5368(3) 0.0446(11) Uani 1 1 d . . .
O9 O 0.3888(3) 0.1611(2) 0.5919(3) 0.0380(10) Uani 1 1 d . . .
O10 O 0.3588(3) 0.2638(2) 0.4292(3) 0.0379(10) Uani 1 1 d . . .
O11 O 0.2560(3) -0.0056(3) 0.5849(4) 0.0479(12) Uani 1 1 d . . .
O12 O 0.2520(4) 0.1130(3) 0.7402(4) 0.0644(14) Uani 1 1 d . . .
O13 O 0.1580(4) 0.1562(3) 0.5679(4) 0.0629(14) Uani 1 1 d . . .
N1 N 0.6088(4) 0.5714(3) 0.7004(4) 0.0389(12) Uani 1 1 d . . .
N2 N 0.5312(4) 0.3290(3) 0.8524(3) 0.0314(11) Uani 1 1 d . . .
N3 N 0.6325(4) 0.2208(3) 0.8195(3) 0.0320(11) Uani 1 1 d . . .
N4 N 0.7897(4) 0.5751(3) 0.5830(3) 0.0342(11) Uani 1 1 d . . .
N5 N 0.8282(4) 0.3042(3) 0.5825(4) 0.0413(13) Uani 1 1 d . . .
N6 N 0.8247(4) 0.2221(3) 0.7096(4) 0.0361(12) Uani 1 1 d . . .


_geom_special_details            
;
All esds (except the esd in the dihedral angle between two l.s. planes)
are estimated using the full covariance matrix. The cell esds are taken
into account individually in the estimation of esds in distances, angles
and torsion angles; correlations between esds in cell parameters are only
used when they are defined by crystal symmetry. An approximate (isotropic)
treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Cu1 N3 1.982(5) . ?
Cu1 N6 2.002(5) . ?
Cu1 N1 2.019(5) 2_646 ?
Cu1 N4 2.041(5) 2_646 ?
Cu1 O6 2.430(4) . ?
Mo1 O8 1.696(4) . ?
Mo1 O10 1.699(4) . ?
Mo1 O3 1.884(4) . ?
Mo1 O9 1.946(4) . ?
Mo1 O5 2.344(4) 3_656 ?
Mo1 O4 2.357(4) . ?
Mo2 O6 1.718(4) . ?
Mo2 O5 1.757(4) . ?
Mo2 O7 1.769(4) . ?
Mo2 O4 1.827(4) . ?
Mo3 O2 1.679(5) . ?
Mo3 O1 1.697(4) . ?
Mo3 O3 1.909(4) . ?
Mo3 O11 1.969(4) 3_656 ?
Mo3 O7 2.277(4) 3_656 ?
Mo3 O4 2.352(4) . ?
Mo4 O12 1.686(5) . ?
Mo4 O13 1.704(5) . ?
Mo4 O11 1.834(4) . ?
Mo4 O9 1.836(4) . ?
C1 N3 1.315(7) . ?
C1 N2 1.329(7) . ?
C1 H1 0.9300 . ?
C2 C3 1.352(8) . ?
C2 N3 1.380(7) . ?
C2 H2 0.9300 . ?
C3 N2 1.369(7) . ?
C3 H3 0.9300 . ?
C4 N2 1.476(7) . ?
C4 C5 1.500(8) . ?
C4 H4A 0.9700 . ?
C4 H4B 0.9700 . ?
C5 C9 1.355(8) . ?
C5 C6 1.403(9) . ?
C6 C7 1.354(10) . ?
C6 H6 0.9300 . ?
C7 C8 1.367(9) . ?
C7 H7 0.9300 . ?
C8 N1 1.351(8) . ?
C8 H8 0.9300 . ?
C9 N1 1.342(8) . ?
C9 H9 0.9300 . ?
C10 N6 1.322(7) . ?
C10 N5 1.329(8) . ?
C10 H10 0.9300 . ?
C11 N6 1.363(8) . ?
C11 C12 1.428(12) . ?
C11 H11 0.9300 . ?
C12 N5 1.379(9) . ?
C12 H12 0.9300 . ?
C13 N5 1.465(8) . ?
C13 C14 1.504(8) . ?
C13 H13A 0.9700 . ?
C13 H13B 0.9700 . ?
C14 C18 1.354(8) . ?
C14 C15 1.371(9) . ?
C15 C16 1.323(10) . ?
C15 H15 0.9300 . ?
C16 C17 1.323(10) . ?
C16 H16 0.9300 . ?
C17 N4 1.334(8) . ?
C17 H17 0.9300 . ?
C18 N4 1.350(7) . ?
C18 H18 0.9300 . ?
O5 Mo1 2.344(4) 3_656 ?
O7 Mo3 2.277(4) 3_656 ?
O11 Mo3 1.969(4) 3_656 ?
N1 Cu1 2.019(5) 2_656 ?
N4 Cu1 2.041(5) 2_656 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
N3 Cu1 N6 93.1(2) . . ?
N3 Cu1 N1 178.2(2) . 2_646 ?
N6 Cu1 N1 88.7(2) . 2_646 ?
N3 Cu1 N4 89.5(2) . 2_646 ?
N6 Cu1 N4 174.7(2) . 2_646 ?
N1 Cu1 N4 88.8(2) 2_646 2_646 ?
N3 Cu1 O6 89.98(17) . . ?
N6 Cu1 O6 95.47(18) . . ?
N1 Cu1 O6 89.41(18) 2_646 . ?
N4 Cu1 O6 89.14(17) 2_646 . ?
O8 Mo1 O10 103.8(2) . . ?
O8 Mo1 O3 99.1(2) . . ?
O10 Mo1 O3 100.72(19) . . ?
O8 Mo1 O9 95.9(2) . . ?
O10 Mo1 O9 101.28(19) . . ?
O3 Mo1 O9 149.47(16) . . ?
O8 Mo1 O5 168.85(17) . 3_656 ?
O10 Mo1 O5 86.94(16) . 3_656 ?
O3 Mo1 O5 81.52(16) . 3_656 ?
O9 Mo1 O5 78.80(16) . 3_656 ?
O8 Mo1 O4 96.71(17) . . ?
O10 Mo1 O4 159.19(16) . . ?
O3 Mo1 O4 72.15(15) . . ?
O9 Mo1 O4 79.82(15) . . ?
O5 Mo1 O4 72.80(14) 3_656 . ?
O6 Mo2 O5 107.17(19) . . ?
O6 Mo2 O7 107.8(2) . . ?
O5 Mo2 O7 110.84(19) . . ?
O6 Mo2 O4 107.4(2) . . ?
O5 Mo2 O4 111.08(18) . . ?
O7 Mo2 O4 112.35(18) . . ?
O2 Mo3 O1 103.7(2) . . ?
O2 Mo3 O3 99.9(2) . . ?
O1 Mo3 O3 101.11(19) . . ?
O2 Mo3 O11 99.5(2) . 3_656 ?
O1 Mo3 O11 93.1(2) . 3_656 ?
O3 Mo3 O11 152.39(18) . 3_656 ?
O2 Mo3 O7 93.9(2) . 3_656 ?
O1 Mo3 O7 161.2(2) . 3_656 ?
O3 Mo3 O7 82.01(16) . 3_656 ?
O11 Mo3 O7 77.24(16) 3_656 3_656 ?
O2 Mo3 O4 165.68(19) . . ?
O1 Mo3 O4 89.6(2) . . ?
O3 Mo3 O4 71.87(15) . . ?
O11 Mo3 O4 84.83(17) 3_656 . ?
O7 Mo3 O4 73.59(15) 3_656 . ?
O12 Mo4 O13 107.8(3) . . ?
O12 Mo4 O11 110.1(2) . . ?
O13 Mo4 O11 106.7(2) . . ?
O12 Mo4 O9 107.9(2) . . ?
O13 Mo4 O9 108.2(2) . . ?
O11 Mo4 O9 115.86(19) . . ?
N3 C1 N2 111.3(5) . . ?
N3 C1 H1 124.3 . . ?
N2 C1 H1 124.3 . . ?
C3 C2 N3 109.7(5) . . ?
C3 C2 H2 125.1 . . ?
N3 C2 H2 125.1 . . ?
C2 C3 N2 105.5(5) . . ?
C2 C3 H3 127.2 . . ?
N2 C3 H3 127.2 . . ?
N2 C4 C5 109.9(5) . . ?
N2 C4 H4A 109.7 . . ?
C5 C4 H4A 109.7 . . ?
N2 C4 H4B 109.7 . . ?
C5 C4 H4B 109.7 . . ?
H4A C4 H4B 108.2 . . ?
C9 C5 C6 117.9(6) . . ?
C9 C5 C4 120.7(6) . . ?
C6 C5 C4 121.4(6) . . ?
C7 C6 C5 119.0(6) . . ?
C7 C6 H6 120.5 . . ?
C5 C6 H6 120.5 . . ?
C6 C7 C8 120.1(6) . . ?
C6 C7 H7 119.9 . . ?
C8 C7 H7 119.9 . . ?
N1 C8 C7 121.6(6) . . ?
N1 C8 H8 119.2 . . ?
C7 C8 H8 119.2 . . ?
N1 C9 C5 123.4(6) . . ?
N1 C9 H9 118.3 . . ?
C5 C9 H9 118.3 . . ?
N6 C10 N5 113.4(6) . . ?
N6 C10 H10 123.3 . . ?
N5 C10 H10 123.3 . . ?
N6 C11 C12 106.2(7) . . ?
N6 C11 H11 126.9 . . ?
C12 C11 H11 126.9 . . ?
N5 C12 C11 107.2(7) . . ?
N5 C12 H12 126.4 . . ?
C11 C12 H12 126.4 . . ?
N5 C13 C14 113.9(5) . . ?
N5 C13 H13A 108.8 . . ?
C14 C13 H13A 108.8 . . ?
N5 C13 H13B 108.8 . . ?
C14 C13 H13B 108.8 . . ?
H13A C13 H13B 107.7 . . ?
C18 C14 C15 118.4(6) . . ?
C18 C14 C13 121.9(6) . . ?
C15 C14 C13 119.5(6) . . ?
C16 C15 C14 121.3(8) . . ?
C16 C15 H15 119.3 . . ?
C14 C15 H15 119.3 . . ?
C17 C16 C15 117.2(8) . . ?
C17 C16 H16 121.4 . . ?
C15 C16 H16 121.4 . . ?
C16 C17 N4 125.2(7) . . ?
C16 C17 H17 117.4 . . ?
N4 C17 H17 117.4 . . ?
N4 C18 C14 121.1(6) . . ?
N4 C18 H18 119.5 . . ?
C14 C18 H18 119.5 . . ?
Mo1 O3 Mo3 122.1(2) . . ?
Mo2 O4 Mo3 134.7(2) . . ?
Mo2 O4 Mo1 134.0(2) . . ?
Mo3 O4 Mo1 89.64(14) . . ?
Mo2 O5 Mo1 123.10(19) . 3_656 ?
Mo2 O6 Cu1 169.7(2) . . ?
Mo2 O7 Mo3 124.4(2) . 3_656 ?
Mo4 O9 Mo1 138.4(2) . . ?
Mo4 O11 Mo3 136.0(3) . 3_656 ?
C9 N1 C8 117.9(5) . . ?
C9 N1 Cu1 120.9(4) . 2_656 ?
C8 N1 Cu1 121.2(4) . 2_656 ?
C1 N2 C3 108.1(5) . . ?
C1 N2 C4 124.7(5) . . ?
C3 N2 C4 126.8(5) . . ?
C1 N3 C2 105.3(5) . . ?
C1 N3 Cu1 126.3(4) . . ?
C2 N3 Cu1 128.4(4) . . ?
C17 N4 C18 116.4(6) . . ?
C17 N4 Cu1 119.9(4) . 2_656 ?
C18 N4 Cu1 123.2(4) . 2_656 ?
C10 N5 C12 105.8(6) . . ?
C10 N5 C13 125.4(5) . . ?
C12 N5 C13 128.5(7) . . ?
C10 N6 C11 107.5(6) . . ?
C10 N6 Cu1 124.8(4) . . ?
C11 N6 Cu1 127.6(5) . . ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
N3 C2 C3 N2 0.1(7) . . . . ?
N2 C4 C5 C9 -106.4(6) . . . . ?
N2 C4 C5 C6 70.9(7) . . . . ?
C9 C5 C6 C7 2.9(10) . . . . ?
C4 C5 C6 C7 -174.5(6) . . . . ?
C5 C6 C7 C8 -2.7(11) . . . . ?
C6 C7 C8 N1 1.8(11) . . . . ?
C6 C5 C9 N1 -2.2(9) . . . . ?
C4 C5 C9 N1 175.2(5) . . . . ?
N6 C11 C12 N5 1.1(8) . . . . ?
N5 C13 C14 C18 -47.6(9) . . . . ?
N5 C13 C14 C15 138.0(7) . . . . ?
C18 C14 C15 C16 0.9(12) . . . . ?
C13 C14 C15 C16 175.5(8) . . . . ?
C14 C15 C16 C17 -5.7(13) . . . . ?
C15 C16 C17 N4 8.1(13) . . . . ?
C15 C14 C18 N4 2.3(10) . . . . ?
C13 C14 C18 N4 -172.2(6) . . . . ?
O8 Mo1 O3 Mo3 74.9(3) . . . . ?
O10 Mo1 O3 Mo3 -179.1(2) . . . . ?
O9 Mo1 O3 Mo3 -43.6(5) . . . . ?
O5 Mo1 O3 Mo3 -93.9(2) 3_656 . . . ?
O4 Mo1 O3 Mo3 -19.3(2) . . . . ?
O2 Mo3 O3 Mo1 -172.7(3) . . . . ?
O1 Mo3 O3 Mo1 -66.5(3) . . . . ?
O11 Mo3 O3 Mo1 53.2(5) 3_656 . . . ?
O7 Mo3 O3 Mo1 94.6(2) 3_656 . . . ?
O4 Mo3 O3 Mo1 19.4(2) . . . . ?
O6 Mo2 O4 Mo3 81.0(3) . . . . ?
O5 Mo2 O4 Mo3 -35.9(3) . . . . ?
O7 Mo2 O4 Mo3 -160.7(3) . . . . ?
O6 Mo2 O4 Mo1 -80.1(3) . . . . ?
O5 Mo2 O4 Mo1 163.0(2) . . . . ?
O7 Mo2 O4 Mo1 38.2(3) . . . . ?
O2 Mo3 O4 Mo2 123.9(7) . . . . ?
O1 Mo3 O4 Mo2 -77.7(3) . . . . ?
O3 Mo3 O4 Mo2 -179.5(3) . . . . ?
O11 Mo3 O4 Mo2 15.5(3) 3_656 . . . ?
O7 Mo3 O4 Mo2 93.7(3) 3_656 . . . ?
O2 Mo3 O4 Mo1 -69.6(8) . . . . ?
O1 Mo3 O4 Mo1 88.85(18) . . . . ?
O3 Mo3 O4 Mo1 -12.97(14) . . . . ?
O11 Mo3 O4 Mo1 -177.96(16) 3_656 . . . ?
O7 Mo3 O4 Mo1 -99.77(15) 3_656 . . . ?
O8 Mo1 O4 Mo2 82.4(3) . . . . ?
O10 Mo1 O4 Mo2 -107.5(5) . . . . ?
O3 Mo1 O4 Mo2 179.8(3) . . . . ?
O9 Mo1 O4 Mo2 -12.5(3) . . . . ?
O5 Mo1 O4 Mo2 -93.8(3) 3_656 . . . ?
O8 Mo1 O4 Mo3 -84.31(19) . . . . ?
O10 Mo1 O4 Mo3 85.9(5) . . . . ?
O3 Mo1 O4 Mo3 13.13(15) . . . . ?
O9 Mo1 O4 Mo3 -179.14(16) . . . . ?
O5 Mo1 O4 Mo3 99.55(15) 3_656 . . . ?
O6 Mo2 O5 Mo1 155.6(2) . . . 3_656 ?
O7 Mo2 O5 Mo1 38.3(3) . . . 3_656 ?
O4 Mo2 O5 Mo1 -87.3(3) . . . 3_656 ?
O5 Mo2 O6 Cu1 165.8(14) . . . . ?
O7 Mo2 O6 Cu1 -74.9(15) . . . . ?
O4 Mo2 O6 Cu1 46.4(15) . . . . ?
N3 Cu1 O6 Mo2 24.6(14) . . . . ?
N6 Cu1 O6 Mo2 -68.5(14) . . . . ?
N1 Cu1 O6 Mo2 -157.1(14) 2_646 . . . ?
N4 Cu1 O6 Mo2 114.1(14) 2_646 . . . ?
O6 Mo2 O7 Mo3 -156.4(2) . . . 3_656 ?
O5 Mo2 O7 Mo3 -39.4(3) . . . 3_656 ?
O4 Mo2 O7 Mo3 85.5(3) . . . 3_656 ?
O12 Mo4 O9 Mo1 -167.4(3) . . . . ?
O13 Mo4 O9 Mo1 -51.0(4) . . . . ?
O11 Mo4 O9 Mo1 68.7(4) . . . . ?
O8 Mo1 O9 Mo4 160.6(3) . . . . ?
O10 Mo1 O9 Mo4 55.2(3) . . . . ?
O3 Mo1 O9 Mo4 -80.1(5) . . . . ?
O5 Mo1 O9 Mo4 -29.3(3) 3_656 . . . ?
O4 Mo1 O9 Mo4 -103.6(3) . . . . ?
O12 Mo4 O11 Mo3 -56.2(4) . . . 3_656 ?
O13 Mo4 O11 Mo3 -172.9(4) . . . 3_656 ?
O9 Mo4 O11 Mo3 66.6(4) . . . 3_656 ?
C5 C9 N1 C8 1.2(9) . . . . ?
C5 C9 N1 Cu1 -177.3(5) . . . 2_656 ?
C7 C8 N1 C9 -1.0(10) . . . . ?
C7 C8 N1 Cu1 177.5(5) . . . 2_656 ?
N3 C1 N2 C3 -1.3(7) . . . . ?
N3 C1 N2 C4 -174.3(5) . . . . ?
C2 C3 N2 C1 0.7(7) . . . . ?
C2 C3 N2 C4 173.6(5) . . . . ?
C5 C4 N2 C1 81.7(7) . . . . ?
C5 C4 N2 C3 -90.0(7) . . . . ?
N2 C1 N3 C2 1.3(7) . . . . ?
N2 C1 N3 Cu1 -177.1(4) . . . . ?
C3 C2 N3 C1 -0.8(7) . . . . ?
C3 C2 N3 Cu1 177.5(4) . . . . ?
N6 Cu1 N3 C1 -63.9(5) . . . . ?
N1 Cu1 N3 C1 130(6) 2_646 . . . ?
N4 Cu1 N3 C1 111.5(5) 2_646 . . . ?
O6 Cu1 N3 C1 -159.4(5) . . . . ?
N6 Cu1 N3 C2 118.1(5) . . . . ?
N1 Cu1 N3 C2 -47(7) 2_646 . . . ?
N4 Cu1 N3 C2 -66.5(5) 2_646 . . . ?
O6 Cu1 N3 C2 22.6(5) . . . . ?
C16 C17 N4 C18 -5.1(11) . . . . ?
C16 C17 N4 Cu1 -177.7(7) . . . 2_656 ?
C14 C18 N4 C17 -0.4(9) . . . . ?
C14 C18 N4 Cu1 172.0(5) . . . 2_656 ?
N6 C10 N5 C12 1.5(7) . . . . ?
N6 C10 N5 C13 175.9(5) . . . . ?
C11 C12 N5 C10 -1.6(8) . . . . ?
C11 C12 N5 C13 -175.7(6) . . . . ?
C14 C13 N5 C10 113.4(7) . . . . ?
C14 C13 N5 C12 -73.6(9) . . . . ?
N5 C10 N6 C11 -0.8(7) . . . . ?
N5 C10 N6 Cu1 -175.9(4) . . . . ?
C12 C11 N6 C10 -0.2(8) . . . . ?
C12 C11 N6 Cu1 174.6(5) . . . . ?
N3 Cu1 N6 C10 -34.4(5) . . . . ?
N1 Cu1 N6 C10 145.2(5) 2_646 . . . ?
N4 Cu1 N6 C10 -153.9(19) 2_646 . . . ?
O6 Cu1 N6 C10 55.9(5) . . . . ?
N3 Cu1 N6 C11 151.6(6) . . . . ?
N1 Cu1 N6 C11 -28.8(6) 2_646 . . . ?
N4 Cu1 N6 C11 32(2) 2_646 . . . ?
O6 Cu1 N6 C11 -118.1(6) . . . . ?

_diffrn_measured_fraction_theta_max 0.995
_diffrn_reflns_theta_full        25.00
_diffrn_measured_fraction_theta_full 0.999
_refine_diff_density_max         0.980
_refine_diff_density_min         -0.748
_refine_diff_density_rms         0.128

